# Electronic Supplementary Material (ESI) for Chemical Science.
# This journal is © The Royal Society of Chemistry 2018

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_NENU_607
_database_code_depnum_ccdc_archive 'CCDC 1855992'
_audit_update_record             
;
2018-07-16 deposited with the CCDC.
2018-10-01 downloaded from the CCDC.
;
_audit_creation_date             2018-07-14
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2014/7
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Mn Mo12 O62 P8, 8(C2 H10 N2), 12(H2 O)'
_chemical_formula_sum            'C16 H104 Mn Mo12 N16 O74 P8'
_chemical_formula_weight         3159.13
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/n 1'
_space_group_name_Hall           '-P 2yn'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   15.8641(14)
_cell_length_b                   15.9370(16)
_cell_length_c                   17.1695(17)
_cell_angle_alpha                90
_cell_angle_beta                 92.645(2)
_cell_angle_gamma                90
_cell_volume                     4336.3(7)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    9951
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.66
_cell_measurement_theta_min      2.56
_shelx_estimated_absorpt_T_max   0.903
_shelx_estimated_absorpt_T_min   0.645
_exptl_absorpt_coefficient_mu    2.088
_exptl_absorpt_correction_T_max  0.7455
_exptl_absorpt_correction_T_min  0.6547
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.0726 before and 0.0449 after correction. The Ratio of minimum to maximum transmission is 0.8782. The λ/2 correction factor is Not present.'
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'clear light red'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    red
_exptl_crystal_density_diffrn    2.420
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       plate
_exptl_crystal_F_000             3106
_exptl_crystal_size_max          0.23
_exptl_crystal_size_mid          0.17
_exptl_crystal_size_min          0.05
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0426
_diffrn_reflns_av_unetI/netI     0.0382
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.985
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            57163
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.985
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.721
_diffrn_reflns_theta_min         1.744
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.985
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                8174
_reflns_number_total             10042
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT v8.37A (Bruker, 2015)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT v8.37A (Bruker, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL (Sheldrick, 2008)'
_computing_structure_solution    'XT (Sheldrick, 2015)'
_refine_diff_density_max         1.276
_refine_diff_density_min         -1.177
_refine_diff_density_rms         0.309
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.186
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     609
_refine_ls_number_reflns         10042
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0625
_refine_ls_R_factor_gt           0.0418
_refine_ls_restrained_S_all      1.186
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0550P)²+13.1341P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0985
_refine_ls_wR_factor_ref         0.1144
_refine_special_details          ?
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H,H) groups, All N(H,H,H) groups
 At 1.5 times of:
  All O(H,H) groups
2. Others
 Fixed Sof: O5W(0.5) H5WA(0.5) H5WB(0.5) O1W(0.5) H1WA(0.5) H1WB(0.5) O6W(0.5)
 H6WA(0.5) H6WB(0.5) O8W(0.5) H8WA(0.5) H8WB(0.5)
3.a Riding coordinates:
 O4W(H4WA,H4WB), O5W(H5WA,H5WB), O1W(H1WA,H1WB), O6W(H6WA,H6WB), O8W(H8WA,H8WB)
3.b Free rotating group:
 O3W(H3WA,H3WB), O7W(H7WA,H7WB), O2W(H2WA,H2WB)
3.c Secondary CH2 refined with riding coordinates:
 C1(H1A,H1B), C6(H6D,H6E), C5(H5D,H5E), C3(H3D,H3E), C2(H2D,H2E), C8(H8D,H8E),
 C7(H7A,H7B), C4(H4D,H4E)
3.d Idealised Me refined as rotating group:
 N6(H6A,H6B,H6C), N8(H8A,H8B,H8C), N1(H1C,H1D,H1E), N5(H5A,H5B,H5C), N3(H3A,
 H3B,H3C), N4(H4A,H4B,H4C), N2(H2A,H2B,H2C), N7(H7C,H7D,H7E)
;
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.57275(3) 0.50502(3) 0.71619(3) 0.01288(11) Uani 1 1 d . . . . .
Mo6 Mo 0.36986(3) 0.42819(3) 0.67117(3) 0.01342(11) Uani 1 1 d . . . . .
Mo2 Mo 0.69900(3) 0.46182(3) 0.63429(3) 0.01319(11) Uani 1 1 d . . . . .
Mo3 Mo 0.66598(3) 0.32746(3) 0.47498(3) 0.01417(11) Uani 1 1 d . . . . .
Mo4 Mo 0.51503(3) 0.26839(3) 0.44428(3) 0.01455(11) Uani 1 1 d . . . . .
Mo5 Mo 0.34395(3) 0.32609(3) 0.55401(3) 0.01395(11) Uani 1 1 d . . . . .
Mn1 Mn 0.5000 0.5000 0.5000 0.0158(2) Uani 1 2 d S T P . .
P1 P 0.54638(8) 0.30888(9) 0.63719(8) 0.0129(3) Uani 1 1 d . . . . .
P4 P 0.43995(9) 0.46059(10) 0.85270(8) 0.0185(3) Uani 1 1 d . . . . .
P3 P 0.36746(10) 0.13105(10) 0.48887(9) 0.0226(3) Uani 1 1 d . . . . .
P2 P 0.84032(8) 0.31956(10) 0.58881(9) 0.0181(3) Uani 1 1 d . . . . .
O2 O 0.5557(2) 0.3851(2) 0.4568(2) 0.0151(8) Uani 1 1 d . . . . .
O9 O 0.4453(2) 0.5356(2) 0.6898(2) 0.0151(8) Uani 1 1 d . . . . .
O5 O 0.7126(2) 0.4437(2) 0.5142(2) 0.0158(8) Uani 1 1 d . . . . .
O3 O 0.5877(2) 0.5110(2) 0.6032(2) 0.0139(7) Uani 1 1 d . . . . .
O1 O 0.3966(2) 0.4383(2) 0.5607(2) 0.0144(7) Uani 1 1 d . . . . .
O19 O 0.5628(2) 0.2340(3) 0.6885(2) 0.0225(9) Uani 1 1 d . . . . .
O17 O 0.4829(2) 0.2884(2) 0.5679(2) 0.0158(8) Uani 1 1 d . . . . .
O8 O 0.3442(2) 0.3092(2) 0.6662(2) 0.0189(8) Uani 1 1 d . . . . .
O26 O 0.3715(3) 0.0488(3) 0.5337(3) 0.0293(10) Uani 1 1 d . . . . .
O18 O 0.5074(2) 0.3836(2) 0.6816(2) 0.0158(8) Uani 1 1 d . . . . .
O7 O 0.3916(2) 0.3202(2) 0.4412(2) 0.0160(8) Uani 1 1 d . . . . .
O28 O 0.3870(2) 0.4116(3) 0.7890(2) 0.0212(9) Uani 1 1 d . . . . .
O30 O 0.4431(3) 0.4086(3) 0.9266(2) 0.0269(10) Uani 1 1 d . . . . .
O25 O 0.3310(2) 0.1993(3) 0.5423(3) 0.0241(9) Uani 1 1 d . . . . .
O21 O 0.7720(2) 0.2809(3) 0.5317(2) 0.0222(9) Uani 1 1 d . . . . .
O10 O 0.6030(2) 0.6021(3) 0.7451(2) 0.0213(8) Uani 1 1 d . . . . .
O4 O 0.6694(2) 0.4331(2) 0.7400(2) 0.0169(8) Uani 1 1 d . . . . .
O29 O 0.5317(2) 0.4706(3) 0.8244(2) 0.0207(8) Uani 1 1 d . . . . .
O20 O 0.7958(2) 0.3767(3) 0.6482(2) 0.0218(9) Uani 1 1 d . . . . .
O6 O 0.6181(2) 0.2153(2) 0.4841(2) 0.0193(8) Uani 1 1 d . . . . .
O31 O 0.4013(3) 0.5469(3) 0.8654(3) 0.0287(10) Uani 1 1 d . . . . .
O16 O 0.6282(2) 0.3420(2) 0.6012(2) 0.0155(8) Uani 1 1 d . . . . .
O24 O 0.4587(3) 0.1565(3) 0.4689(3) 0.0253(9) Uani 1 1 d . . . . .
O13 O 0.5157(3) 0.2555(3) 0.3458(2) 0.0253(9) Uani 1 1 d . . . . .
O22 O 0.8832(2) 0.2479(3) 0.6350(3) 0.0269(10) Uani 1 1 d . . . . .
O12 O 0.7022(3) 0.3297(3) 0.3843(2) 0.0259(9) Uani 1 1 d . . . . .
O11 O 0.7586(2) 0.5488(3) 0.6442(3) 0.0249(9) Uani 1 1 d . . . . .
O15 O 0.2749(2) 0.4757(3) 0.6719(2) 0.0246(9) Uani 1 1 d . . . . .
O14 O 0.2438(2) 0.3511(3) 0.5272(2) 0.0248(9) Uani 1 1 d . . . . .
O27 O 0.3152(3) 0.1204(3) 0.4130(3) 0.0413(12) Uani 1 1 d . . . . .
O23 O 0.9037(3) 0.3697(3) 0.5441(3) 0.0310(10) Uani 1 1 d . . . . .
N6 N 0.3690(3) 0.4130(4) 1.0665(3) 0.0284(12) Uani 1 1 d . . . . .
H6A H 0.3980 0.4125 1.0234 0.034 Uiso 1 1 calc GR . . . .
H6B H 0.3733 0.3632 1.0897 0.034 Uiso 1 1 calc GR . . . .
H6C H 0.3896 0.4525 1.0987 0.034 Uiso 1 1 calc GR . . . .
N8 N 1.0444(3) 0.2019(4) 0.6868(3) 0.0313(12) Uani 1 1 d . . . . .
H8A H 1.0003 0.2195 0.6572 0.038 Uiso 1 1 calc GR . . . .
H8B H 1.0324 0.2058 0.7368 0.038 Uiso 1 1 calc GR . . . .
H8C H 1.0557 0.1488 0.6754 0.038 Uiso 1 1 calc GR . . . .
C1 C 0.2367(4) 0.2650(4) 0.2786(4) 0.0322(15) Uani 1 1 d . . . . .
H1A H 0.2088 0.2322 0.2373 0.039 Uiso 1 1 calc R . . . .
H1B H 0.2399 0.3224 0.2604 0.039 Uiso 1 1 calc R . . . .
N1 N 0.3231(3) 0.2326(4) 0.2927(3) 0.0406(15) Uani 1 1 d . . . . .
H1C H 0.3471 0.2256 0.2473 0.049 Uiso 1 1 calc GR . . . .
H1D H 0.3211 0.1836 0.3174 0.049 Uiso 1 1 calc GR . . . .
H1E H 0.3531 0.2690 0.3218 0.049 Uiso 1 1 calc GR . . . .
N5 N 0.1350(4) 0.4146(4) 1.0895(4) 0.0452(16) Uani 1 1 d . . . . .
H5A H 0.1215 0.3680 1.0632 0.054 Uiso 1 1 calc GR . . . .
H5B H 0.1248 0.4590 1.0591 0.054 Uiso 1 1 calc GR . . . .
H5C H 0.1042 0.4180 1.1314 0.054 Uiso 1 1 calc GR . . . .
C6 C 0.2799(4) 0.4309(5) 1.0461(4) 0.0317(15) Uani 1 1 d . . . . .
H6D H 0.2613 0.3969 1.0017 0.038 Uiso 1 1 calc R . . . .
H6E H 0.2737 0.4894 1.0314 0.038 Uiso 1 1 calc R . . . .
N3 N 0.2738(4) 0.0418(4) 0.6632(4) 0.0369(14) Uani 1 1 d . . . . .
H3A H 0.2958 0.0476 0.6168 0.044 Uiso 1 1 calc GR . . . .
H3B H 0.2178 0.0412 0.6575 0.044 Uiso 1 1 calc GR . . . .
H3C H 0.2916 -0.0061 0.6849 0.044 Uiso 1 1 calc GR . . . .
N4 N 0.4242(4) 0.1910(4) 0.7664(4) 0.0457(16) Uani 1 1 d . . . . .
H4A H 0.4771 0.2024 0.7550 0.055 Uiso 1 1 calc GR . . . .
H4B H 0.4216 0.1825 0.8175 0.055 Uiso 1 1 calc GR . . . .
H4C H 0.3912 0.2341 0.7523 0.055 Uiso 1 1 calc GR . . . .
N2 N 0.1626(4) 0.1775(4) 0.3720(4) 0.0485(18) Uani 1 1 d . . . . .
H2A H 0.1375 0.1506 0.3319 0.058 Uiso 1 1 calc GR . . . .
H2B H 0.1279 0.1796 0.4112 0.058 Uiso 1 1 calc GR . . . .
H2C H 0.2095 0.1503 0.3873 0.058 Uiso 1 1 calc GR . . . .
C5 C 0.2253(4) 0.4124(5) 1.1139(4) 0.0373(16) Uani 1 1 d . . . . .
H5D H 0.2394 0.3574 1.1350 0.045 Uiso 1 1 calc R . . . .
H5E H 0.2364 0.4535 1.1547 0.045 Uiso 1 1 calc R . . . .
O4W O 0.4849(5) -0.0323(5) 0.6273(4) 0.087(3) Uani 1 1 d . . . . .
H4WA H 0.4500 -0.0141 0.5922 0.130 Uiso 1 1 d R . . . .
H4WB H 0.4852 -0.0851 0.6206 0.130 Uiso 1 1 d R . . . .
C3 C 0.3009(4) 0.1134(4) 0.7143(4) 0.0336(15) Uani 1 1 d . . . . .
H3D H 0.2766 0.1075 0.7649 0.040 Uiso 1 1 calc R . . . .
H3E H 0.2808 0.1657 0.6913 0.040 Uiso 1 1 calc R . . . .
O3W O 0.7088(6) 0.1368(5) 0.3304(5) 0.086(2) Uani 1 1 d . . . . .
H3WA H 0.6569 0.1415 0.3399 0.129 Uiso 1 1 d G . . . .
H3WB H 0.7297 0.1852 0.3237 0.129 Uiso 1 1 d G . . . .
C2 C 0.1839(4) 0.2627(5) 0.3485(4) 0.0379(17) Uani 1 1 d . . . . .
H2D H 0.2141 0.2905 0.3916 0.046 Uiso 1 1 calc R . . . .
H2E H 0.1322 0.2938 0.3370 0.046 Uiso 1 1 calc R . . . .
O7W O 0.5782(6) 0.3535(7) 1.0078(5) 0.123(4) Uani 1 1 d . . . . .
H7WA H 0.6049 0.3989 1.0171 0.184 Uiso 1 1 d G . . . .
H7WB H 0.5304 0.3647 0.9858 0.184 Uiso 1 1 d G . . . .
C8 C 1.1184(5) 0.2547(5) 0.6721(6) 0.048(2) Uani 1 1 d . . . . .
H8D H 1.1451 0.2331 0.6265 0.058 Uiso 1 1 calc R . . . .
H8E H 1.1587 0.2493 0.7161 0.058 Uiso 1 1 calc R . . . .
C7 C 1.0999(6) 0.3447(6) 0.6596(6) 0.060(2) Uani 1 1 d . . . . .
H7A H 1.0591 0.3621 0.6968 0.072 Uiso 1 1 calc R . . . .
H7B H 1.1512 0.3764 0.6709 0.072 Uiso 1 1 calc R . . . .
C4 C 0.3954(4) 0.1154(5) 0.7243(5) 0.0426(18) Uani 1 1 d . . . . .
H4D H 0.4148 0.0660 0.7529 0.051 Uiso 1 1 calc R . . . .
H4E H 0.4196 0.1142 0.6734 0.051 Uiso 1 1 calc R . . . .
O2W O 0.8784(5) 0.4573(8) 0.4113(6) 0.118(4) Uani 1 1 d . . . . .
H2WA H 0.8983 0.4611 0.4580 0.177 Uiso 1 1 d G . . . .
H2WB H 0.8264 0.4701 0.4094 0.177 Uiso 1 1 d G . . . .
N7 N 1.0676(5) 0.3669(9) 0.5821(6) 0.128(5) Uani 1 1 d . . . . .
H7C H 1.0797 0.3263 0.5489 0.153 Uiso 1 1 calc GR . . . .
H7D H 1.0912 0.4146 0.5674 0.153 Uiso 1 1 calc GR . . . .
H7E H 1.0119 0.3735 0.5824 0.153 Uiso 1 1 calc GR . . . .
O5W O 0.3517(12) 0.2688(9) 0.8906(8) 0.095(6) Uani 0.5 1 d . . . A 1
H5WA H 0.3870 0.3001 0.9155 0.142 Uiso 0.5 1 d R . . A 1
H5WB H 0.3369 0.2330 0.9240 0.142 Uiso 0.5 1 d R . . A 1
O1W O 1.0660(10) 0.4408(11) 0.4195(12) 0.125(8) Uani 0.5 1 d . . . . .
H1WA H 1.1107 0.4485 0.3951 0.188 Uiso 0.5 1 d R . . . .
H1WB H 1.0552 0.4885 0.4388 0.188 Uiso 0.5 1 d R . . . .
O6W O 0.4650(14) 0.2330(9) 0.9187(8) 0.105(7) Uani 0.5 1 d . . . B 2
H6WA H 0.5051 0.1989 0.9111 0.158 Uiso 0.5 1 d R . . B 2
H6WB H 0.4686 0.2695 0.8829 0.158 Uiso 0.5 1 d R . . B 2
O8W O 0.0770(11) 0.5019(14) 1.2585(12) 0.140(9) Uani 0.5 1 d . . . . .
H8WA H 0.0974 0.5245 1.2187 0.211 Uiso 0.5 1 d R . . . .
H8WB H 0.0325 0.5299 1.2661 0.211 Uiso 0.5 1 d R . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 Mo2 2.5928(6) . ?
Mo1 O9 2.108(4) . ?
Mo1 O3 1.967(4) . ?
Mo1 O18 2.262(4) . ?
Mo1 O10 1.688(4) . ?
Mo1 O4 1.942(4) . ?
Mo1 O29 2.071(4) . ?
Mo6 Mo5 2.6051(7) . ?
Mo6 O9 2.105(4) . ?
Mo6 O1 1.969(4) . ?
Mo6 O8 1.941(4) . ?
Mo6 O18 2.294(3) . ?
Mo6 O28 2.045(4) . ?
Mo6 O15 1.687(4) . ?
Mo2 O5 2.103(4) . ?
Mo2 O3 1.983(3) . ?
Mo2 O4 1.949(4) . ?
Mo2 O20 2.055(4) . ?
Mo2 O16 2.274(4) . ?
Mo2 O11 1.682(4) . ?
Mo3 Mo4 2.6042(6) . ?
Mo3 O2 1.988(3) . ?
Mo3 O5 2.095(4) . ?
Mo3 O21 2.043(4) . ?
Mo3 O6 1.952(4) . ?
Mo3 O16 2.287(4) . ?
Mo3 O12 1.684(4) . ?
Mo4 O2 1.977(4) . ?
Mo4 O17 2.228(4) . ?
Mo4 O7 2.123(4) . ?
Mo4 O6 1.938(4) . ?
Mo4 O24 2.048(4) . ?
Mo4 O13 1.703(4) . ?
Mo5 O1 1.975(4) . ?
Mo5 O17 2.286(3) . ?
Mo5 O8 1.945(4) . ?
Mo5 O7 2.114(4) . ?
Mo5 O25 2.040(4) . ?
Mo5 O14 1.682(4) . ?
Mn1 O2 2.178(4) 3_666 ?
Mn1 O2 2.178(4) . ?
Mn1 O3 2.209(3) . ?
Mn1 O3 2.209(3) 3_666 ?
Mn1 O1 2.213(4) 3_666 ?
Mn1 O1 2.213(4) . ?
P1 O19 1.499(4) . ?
P1 O17 1.558(4) . ?
P1 O18 1.557(4) . ?
P1 O16 1.555(4) . ?
P4 O28 1.558(4) . ?
P4 O30 1.515(4) . ?
P4 O29 1.564(4) . ?
P4 O31 1.525(5) . ?
P3 O26 1.520(5) . ?
P3 O25 1.552(4) . ?
P3 O24 1.556(4) . ?
P3 O27 1.522(5) . ?
P2 O21 1.556(4) . ?
P2 O20 1.561(4) . ?
P2 O22 1.532(4) . ?
P2 O23 1.520(4) . ?
N6 C6 1.468(8) . ?
N8 C8 1.476(9) . ?
C1 N1 1.474(9) . ?
C1 C2 1.495(9) . ?
N5 C5 1.473(9) . ?
C6 C5 1.512(9) . ?
N3 C3 1.491(9) . ?
N4 C4 1.468(9) . ?
N2 C2 1.462(10) . ?
C3 C4 1.501(9) . ?
C8 C7 1.479(12) . ?
C7 N7 1.448(13) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O9 Mo1 Mo2 134.55(10) . . ?
O9 Mo1 O18 73.61(14) . . ?
O3 Mo1 Mo2 49.23(10) . . ?
O3 Mo1 O9 86.24(14) . . ?
O3 Mo1 O18 81.80(14) . . ?
O3 Mo1 O29 162.66(15) . . ?
O18 Mo1 Mo2 89.24(9) . . ?
O10 Mo1 Mo2 100.78(13) . . ?
O10 Mo1 O9 96.21(17) . . ?
O10 Mo1 O3 101.58(17) . . ?
O10 Mo1 O18 169.16(16) . . ?
O10 Mo1 O4 105.55(18) . . ?
O10 Mo1 O29 94.32(18) . . ?
O4 Mo1 Mo2 48.34(11) . . ?
O4 Mo1 O9 157.11(16) . . ?
O4 Mo1 O3 96.08(15) . . ?
O4 Mo1 O18 84.15(15) . . ?
O4 Mo1 O29 86.16(15) . . ?
O29 Mo1 Mo2 134.34(11) . . ?
O29 Mo1 O9 85.20(14) . . ?
O29 Mo1 O18 81.33(15) . . ?
O9 Mo6 Mo5 133.90(10) . . ?
O9 Mo6 O18 73.01(14) . . ?
O1 Mo6 Mo5 48.77(11) . . ?
O1 Mo6 O9 86.15(15) . . ?
O1 Mo6 O18 81.61(14) . . ?
O1 Mo6 O28 159.76(15) . . ?
O8 Mo6 Mo5 47.98(11) . . ?
O8 Mo6 O9 156.64(15) . . ?
O8 Mo6 O1 95.30(16) . . ?
O8 Mo6 O18 84.11(15) . . ?
O8 Mo6 O28 86.26(16) . . ?
O18 Mo6 Mo5 88.99(9) . . ?
O28 Mo6 Mo5 133.77(12) . . ?
O28 Mo6 O9 84.64(15) . . ?
O28 Mo6 O18 78.47(14) . . ?
O15 Mo6 Mo5 100.20(14) . . ?
O15 Mo6 O9 97.82(18) . . ?
O15 Mo6 O1 101.72(18) . . ?
O15 Mo6 O8 104.66(19) . . ?
O15 Mo6 O18 170.14(17) . . ?
O15 Mo6 O28 97.37(18) . . ?
O5 Mo2 Mo1 133.21(10) . . ?
O5 Mo2 O16 73.23(14) . . ?
O3 Mo2 Mo1 48.71(10) . . ?
O3 Mo2 O5 85.43(14) . . ?
O3 Mo2 O20 160.75(16) . . ?
O3 Mo2 O16 80.84(14) . . ?
O4 Mo2 Mo1 48.11(11) . . ?
O4 Mo2 O5 156.99(16) . . ?
O4 Mo2 O3 95.35(15) . . ?
O4 Mo2 O20 87.00(16) . . ?
O4 Mo2 O16 84.16(15) . . ?
O20 Mo2 Mo1 134.76(12) . . ?
O20 Mo2 O5 85.07(15) . . ?
O20 Mo2 O16 80.40(14) . . ?
O16 Mo2 Mo1 88.48(9) . . ?
O11 Mo2 Mo1 99.85(14) . . ?
O11 Mo2 O5 97.44(18) . . ?
O11 Mo2 O3 101.02(18) . . ?
O11 Mo2 O4 104.94(19) . . ?
O11 Mo2 O20 96.79(18) . . ?
O11 Mo2 O16 170.40(17) . . ?
O2 Mo3 Mo4 48.77(11) . . ?
O2 Mo3 O5 86.36(14) . . ?
O2 Mo3 O21 160.34(16) . . ?
O2 Mo3 O16 80.48(14) . . ?
O5 Mo3 Mo4 133.81(10) . . ?
O5 Mo3 O16 73.11(14) . . ?
O21 Mo3 Mo4 133.94(12) . . ?
O21 Mo3 O5 84.15(15) . . ?
O21 Mo3 O16 80.30(14) . . ?
O6 Mo3 Mo4 47.74(11) . . ?
O6 Mo3 O2 95.34(15) . . ?
O6 Mo3 O5 156.58(15) . . ?
O6 Mo3 O21 86.78(16) . . ?
O6 Mo3 O16 84.11(15) . . ?
O16 Mo3 Mo4 87.11(9) . . ?
O12 Mo3 Mo4 99.81(14) . . ?
O12 Mo3 O2 100.40(18) . . ?
O12 Mo3 O5 98.52(18) . . ?
O12 Mo3 O21 98.00(18) . . ?
O12 Mo3 O6 104.10(19) . . ?
O12 Mo3 O16 171.56(18) . . ?
O2 Mo4 Mo3 49.13(10) . . ?
O2 Mo4 O17 81.37(14) . . ?
O2 Mo4 O7 86.13(14) . . ?
O2 Mo4 O24 160.12(16) . . ?
O17 Mo4 Mo3 90.25(9) . . ?
O7 Mo4 Mo3 134.64(10) . . ?
O7 Mo4 O17 73.56(13) . . ?
O6 Mo4 Mo3 48.19(12) . . ?
O6 Mo4 O2 96.14(15) . . ?
O6 Mo4 O17 87.33(15) . . ?
O6 Mo4 O7 160.23(15) . . ?
O6 Mo4 O24 85.20(17) . . ?
O24 Mo4 Mo3 132.79(12) . . ?
O24 Mo4 O17 78.87(15) . . ?
O24 Mo4 O7 86.16(16) . . ?
O13 Mo4 Mo3 101.33(14) . . ?
O13 Mo4 O2 101.77(18) . . ?
O13 Mo4 O17 167.06(16) . . ?
O13 Mo4 O7 94.01(17) . . ?
O13 Mo4 O6 104.67(18) . . ?
O13 Mo4 O24 97.03(19) . . ?
O1 Mo5 Mo6 48.56(10) . . ?
O1 Mo5 O17 80.13(14) . . ?
O1 Mo5 O7 85.71(14) . . ?
O1 Mo5 O25 160.57(15) . . ?
O17 Mo5 Mo6 88.10(9) . . ?
O8 Mo5 Mo6 47.83(12) . . ?
O8 Mo5 O1 94.95(15) . . ?
O8 Mo5 O17 84.42(15) . . ?
O8 Mo5 O7 156.51(15) . . ?
O8 Mo5 O25 87.48(17) . . ?
O7 Mo5 Mo6 133.23(10) . . ?
O7 Mo5 O17 72.53(13) . . ?
O25 Mo5 Mo6 134.94(12) . . ?
O25 Mo5 O17 80.93(15) . . ?
O25 Mo5 O7 84.52(16) . . ?
O14 Mo5 Mo6 100.18(15) . . ?
O14 Mo5 O1 101.17(18) . . ?
O14 Mo5 O17 170.05(17) . . ?
O14 Mo5 O8 105.20(19) . . ?
O14 Mo5 O7 97.66(17) . . ?
O14 Mo5 O25 96.75(19) . . ?
O2 Mn1 O2 180.00(10) 3_666 . ?
O2 Mn1 O3 95.15(13) 3_666 3_666 ?
O2 Mn1 O3 84.85(13) 3_666 . ?
O2 Mn1 O3 84.85(13) . 3_666 ?
O2 Mn1 O3 95.15(13) . . ?
O2 Mn1 O1 83.80(13) 3_666 . ?
O2 Mn1 O1 96.20(13) . . ?
O2 Mn1 O1 83.79(13) . 3_666 ?
O2 Mn1 O1 96.21(13) 3_666 3_666 ?
O3 Mn1 O3 180.0 3_666 . ?
O3 Mn1 O1 83.68(13) 3_666 . ?
O3 Mn1 O1 96.32(13) . . ?
O3 Mn1 O1 96.32(13) 3_666 3_666 ?
O3 Mn1 O1 83.68(13) . 3_666 ?
O1 Mn1 O1 180.0 . 3_666 ?
O19 P1 O17 111.8(2) . . ?
O19 P1 O18 112.5(2) . . ?
O19 P1 O16 112.3(2) . . ?
O18 P1 O17 106.1(2) . . ?
O16 P1 O17 106.8(2) . . ?
O16 P1 O18 107.0(2) . . ?
O28 P4 O29 108.2(2) . . ?
O30 P4 O28 108.1(2) . . ?
O30 P4 O29 108.7(2) . . ?
O30 P4 O31 111.8(3) . . ?
O31 P4 O28 110.2(2) . . ?
O31 P4 O29 109.8(2) . . ?
O26 P3 O25 108.2(3) . . ?
O26 P3 O24 108.6(2) . . ?
O26 P3 O27 110.3(3) . . ?
O25 P3 O24 108.9(2) . . ?
O27 P3 O25 112.4(3) . . ?
O27 P3 O24 108.4(3) . . ?
O21 P2 O20 108.7(2) . . ?
O22 P2 O21 108.1(2) . . ?
O22 P2 O20 107.5(2) . . ?
O23 P2 O21 110.4(2) . . ?
O23 P2 O20 110.6(3) . . ?
O23 P2 O22 111.4(2) . . ?
Mo3 O2 Mn1 134.65(18) . . ?
Mo4 O2 Mo3 82.10(14) . . ?
Mo4 O2 Mn1 133.82(18) . . ?
Mo6 O9 Mo1 112.21(17) . . ?
Mo3 O5 Mo2 112.70(17) . . ?
Mo1 O3 Mo2 82.06(13) . . ?
Mo1 O3 Mn1 133.42(18) . . ?
Mo2 O3 Mn1 134.81(18) . . ?
Mo6 O1 Mo5 82.66(14) . . ?
Mo6 O1 Mn1 133.43(18) . . ?
Mo5 O1 Mn1 134.06(18) . . ?
Mo4 O17 Mo5 101.57(14) . . ?
P1 O17 Mo4 126.1(2) . . ?
P1 O17 Mo5 127.6(2) . . ?
Mo6 O8 Mo5 84.18(15) . . ?
Mo1 O18 Mo6 100.25(14) . . ?
P1 O18 Mo1 126.5(2) . . ?
P1 O18 Mo6 126.6(2) . . ?
Mo5 O7 Mo4 111.25(16) . . ?
P4 O28 Mo6 132.2(2) . . ?
P3 O25 Mo5 135.5(2) . . ?
P2 O21 Mo3 133.7(2) . . ?
Mo1 O4 Mo2 83.56(14) . . ?
P4 O29 Mo1 129.9(2) . . ?
P2 O20 Mo2 131.9(2) . . ?
Mo4 O6 Mo3 84.07(15) . . ?
Mo2 O16 Mo3 100.03(14) . . ?
P1 O16 Mo2 126.7(2) . . ?
P1 O16 Mo3 127.0(2) . . ?
P3 O24 Mo4 133.8(3) . . ?
N1 C1 C2 114.3(6) . . ?
N6 C6 C5 111.0(5) . . ?
N5 C5 C6 111.1(6) . . ?
N3 C3 C4 110.0(6) . . ?
N2 C2 C1 112.9(6) . . ?
N8 C8 C7 115.0(6) . . ?
N7 C7 C8 115.5(10) . . ?
N4 C4 C3 111.1(6) . . ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_NENU_605
_database_code_depnum_ccdc_archive 'CCDC 1855993'
_audit_update_record             
;
2018-07-16 deposited with the CCDC.
2018-10-01 downloaded from the CCDC.
;
_audit_creation_date             2018-07-15
_audit_creation_method           
;
Olex2 1.2
(compiled 2017.08.10 svn.r3458 for OlexSys, GUI svn.r5486)
;
_shelx_SHELXL_version_number     2014/7
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         '0.5(K32 Mn80 Mo192 Na16 O1088 P136), 16(O)'
_chemical_formula_sum            'K16 Mn40 Mo96 Na8 O560 P68'
_chemical_formula_weight         23283.32
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      tetragonal
_space_group_IT_number           142
_space_group_name_H-M_alt        'I 41/a c d'
_space_group_name_Hall           '-I 4bd 2c'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-y+1/4, x+3/4, z+1/4'
'y+1/4, -x+1/4, z+3/4'
'-x+1/2, y, -z'
'x, -y, -z+1/2'
'y+1/4, x+3/4, -z+3/4'
'-y+1/4, -x+1/4, -z+1/4'
'x+1/2, y+1/2, z+1/2'
'-x+1, -y+1/2, z+1'
'-y+3/4, x+5/4, z+3/4'
'y+3/4, -x+3/4, z+5/4'
'-x+1, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1'
'y+3/4, x+5/4, -z+5/4'
'-y+3/4, -x+3/4, -z+3/4'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'y-1/4, -x-3/4, -z-1/4'
'-y-1/4, x-1/4, -z-3/4'
'x-1/2, -y, z'
'-x, y, z-1/2'
'-y-1/4, -x-3/4, z-3/4'
'y-1/4, x-1/4, z-1/4'
'-x+1/2, -y+1/2, -z+1/2'
'x, y+1/2, -z'
'y+1/4, -x-1/4, -z+1/4'
'-y+1/4, x+1/4, -z-1/4'
'x, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z'
'-y+1/4, -x-1/4, z-1/4'
'y+1/4, x+1/4, z+1/4'

_cell_length_a                   27.4698(12)
_cell_length_b                   27.4698(12)
_cell_length_c                   39.881(3)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     30093(4)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    9756
_cell_measurement_temperature    300(2)
_cell_measurement_theta_max      25.659
_cell_measurement_theta_min      2.257
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    3.141
_exptl_absorpt_correction_T_max  0.763
_exptl_absorpt_correction_T_min  0.562
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
'SADABS-2014/5 (Bruker,2014/5) was used for absorption correction.'
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'clear reddish red'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   reddish
_exptl_crystal_colour_primary    red
_exptl_crystal_density_diffrn    2.570
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       plate
_exptl_crystal_F_000             21848
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.1
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0619
_diffrn_reflns_av_unetI/netI     0.0297
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       33
_diffrn_reflns_limit_h_min       -33
_diffrn_reflns_limit_k_max       33
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       48
_diffrn_reflns_limit_l_min       -48
_diffrn_reflns_number            91557
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         25.703
_diffrn_reflns_theta_min         2.928
_diffrn_ambient_temperature      300.27
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  CMOS-PHOTON100
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                5413
_reflns_number_total             7150
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT v8.37A (Bruker, 2015)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT v8.37A (Bruker, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'olex2.solve (Bourhis et al., 2015)'
_refine_diff_density_max         1.247
_refine_diff_density_min         -1.140
_refine_diff_density_rms         0.205
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.089
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     445
_refine_ls_number_reflns         7150
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0747
_refine_ls_R_factor_gt           0.0479
_refine_ls_restrained_S_all      1.089
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0506P)²+1071.1046P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1149
_refine_ls_wR_factor_ref         0.1360
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     iterative
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.68033(3) 0.59776(3) 0.46771(2) 0.01987(17) Uani 1 1 d . . . . .
Mo2 Mo 0.71817(3) 0.64482(3) 0.41769(2) 0.02012(17) Uani 1 1 d . . . . .
Mo3 Mo 0.72027(3) 0.77159(3) 0.41738(2) 0.02185(18) Uani 1 1 d . . . . .
Mo4 Mo 0.68170(3) 0.81952(3) 0.46717(2) 0.02123(18) Uani 1 1 d . . . . .
Mo5 Mo 0.62645(3) 0.75725(3) 0.53378(2) 0.02163(18) Uani 1 1 d . . . . .
Mo6 Mo 0.62539(3) 0.66305(3) 0.53313(2) 0.02161(18) Uani 1 1 d . . . . .
Mn3 Mn 0.7500 0.70850(6) 0.5000 0.0206(4) Uani 1 2 d S T P . .
Mn1 Mn 0.52186(5) 0.65967(6) 0.43212(4) 0.0342(4) Uani 1 1 d . . . . .
Mn2 Mn 0.53859(6) 0.95873(5) 0.48243(4) 0.0381(4) Uani 1 1 d . . . . .
K0AA K 0.58307(8) 0.81833(10) 0.41253(6) 0.0443(6) Uani 1 1 d . . . . .
P1 P 0.62577(7) 0.70969(7) 0.45439(6) 0.0184(4) Uani 1 1 d . . . . .
P2 P 0.56658(8) 0.57758(8) 0.49035(6) 0.0247(5) Uani 1 1 d . . . . .
P3 P 0.68696(9) 0.70812(8) 0.34902(6) 0.0258(5) Uani 1 1 d . . . . .
P4 P 0.56802(9) 0.84358(8) 0.49101(6) 0.0259(5) Uani 1 1 d . . . . .
P5 P 0.5000 0.7500 0.3750 0.0380(12) Uani 1 4 d S T P . .
Na1 Na 0.5000 0.7500 0.4953(2) 0.0631(19) Uani 1 2 d S T P . .
O1 O 0.6310(2) 0.6638(2) 0.47688(16) 0.0229(13) Uani 1 1 d . . . . .
O2 O 0.6681(2) 0.70910(19) 0.42889(15) 0.0212(12) Uani 1 1 d . . . . .
O3 O 0.6333(2) 0.7550(2) 0.47696(15) 0.0223(13) Uani 1 1 d . . . . .
O4 O 0.5766(2) 0.7127(2) 0.43808(17) 0.0303(15) Uani 1 1 d . . . . .
O5 O 0.7299(2) 0.6493(2) 0.46629(14) 0.0202(12) Uani 1 1 d . . . . .
O6 O 0.6797(2) 0.7094(2) 0.52944(15) 0.0215(12) Uani 1 1 d . . . . .
O7 O 0.7315(2) 0.7672(2) 0.46610(14) 0.0215(12) Uani 1 1 d . . . . .
O8 O 0.7610(2) 0.7080(2) 0.41406(15) 0.0242(13) Uani 1 1 d . . . . .
O9 O 0.6775(2) 0.6101(2) 0.51938(15) 0.0215(12) Uani 1 1 d . . . . .
O10 O 0.6789(2) 0.8103(2) 0.51958(16) 0.0263(14) Uani 1 1 d . . . . .
O11 O 0.6992(2) 0.7545(2) 0.36953(16) 0.0300(14) Uani 1 1 d . . . . .
O12 O 0.6959(2) 0.6624(2) 0.37006(16) 0.0291(14) Uani 1 1 d . . . . .
O13 O 0.6590(2) 0.6067(2) 0.42197(15) 0.0238(13) Uani 1 1 d . . . . .
O14 O 0.6169(2) 0.5596(2) 0.47749(17) 0.0281(14) Uani 1 1 d . . . . .
O15 O 0.5743(2) 0.6113(2) 0.52033(16) 0.0270(14) Uani 1 1 d . . . . .
O16 O 0.5742(2) 0.7108(2) 0.52606(15) 0.0260(13) Uani 1 1 d . . . . .
O17 O 0.5765(2) 0.8099(2) 0.52112(16) 0.0283(14) Uani 1 1 d . . . . .
O18 O 0.6163(2) 0.8532(2) 0.47245(17) 0.0357(16) Uani 1 1 d . . . . .
O19 O 0.6612(2) 0.8104(2) 0.42109(15) 0.0243(13) Uani 1 1 d . . . . .
O019 O 0.5724(3) 0.6296(3) 0.3918(2) 0.0453(19) Uani 1 1 d . . . . .
O20 O 0.7640(2) 0.8110(2) 0.40615(17) 0.0331(15) Uani 1 1 d . . . . .
O21 O 0.7608(2) 0.6049(2) 0.40595(16) 0.0310(15) Uani 1 1 d . . . . .
O22 O 0.7151(2) 0.5477(2) 0.46751(16) 0.0294(14) Uani 1 1 d . . . . .
O23 O 0.6250(2) 0.6513(2) 0.57430(17) 0.0348(16) Uani 1 1 d . . . . .
O24 O 0.6268(2) 0.7687(2) 0.57514(16) 0.0319(15) Uani 1 1 d . . . . .
O25 O 0.7167(2) 0.8694(2) 0.46684(17) 0.0331(15) Uani 1 1 d . . . . .
O26 O 0.5368(2) 0.5334(2) 0.50145(18) 0.0346(16) Uani 1 1 d . . . . .
O27 O 0.5394(2) 0.6007(3) 0.46164(19) 0.0409(17) Uani 1 1 d . . . . .
O28 O 0.7194(3) 0.7059(3) 0.31822(19) 0.0458(19) Uani 1 1 d . . . . .
O29 O 0.6341(3) 0.7101(3) 0.3389(2) 0.0457(19) Uani 1 1 d . . . . .
O30 O 0.5479(2) 0.8914(2) 0.50452(18) 0.0365(16) Uani 1 1 d . . . . .
O31 O 0.5339(3) 0.8176(2) 0.46649(17) 0.0371(16) Uani 1 1 d . . . . .
O32 O 0.5155(3) 0.7930(3) 0.3963(2) 0.054(2) Uani 1 1 d . . . . .
O33 O 0.6200(3) 0.9678(3) 0.4943(2) 0.058(2) Uani 1 1 d . . . . .
O1W O 0.6755(4) 0.9138(4) 0.5381(3) 0.094(4) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 Mo2 2.5945(11) . ?
Mo1 O1 2.293(5) . ?
Mo1 O5 1.964(5) . ?
Mo1 O9 2.090(6) . ?
Mo1 O13 1.932(6) . ?
Mo1 O14 2.070(6) . ?
Mo1 O22 1.675(6) . ?
Mo2 O2 2.283(5) . ?
Mo2 O5 1.968(6) . ?
Mo2 O8 2.101(6) . ?
Mo2 O12 2.053(6) . ?
Mo2 O13 1.942(6) . ?
Mo2 O21 1.670(6) . ?
Mo3 Mo4 2.6075(11) . ?
Mo3 K0AA 3.986(2) . ?
Mo3 O2 2.283(6) . ?
Mo3 O7 1.971(6) . ?
Mo3 O8 2.079(6) . ?
Mo3 O11 2.049(6) . ?
Mo3 O19 1.946(6) . ?
Mo3 O20 1.678(6) . ?
Mo4 K0AA 3.477(2) . ?
Mo4 O3 2.249(6) . ?
Mo4 O7 1.984(6) . ?
Mo4 O10 2.107(6) . ?
Mo4 O18 2.032(7) . ?
Mo4 O19 1.938(6) . ?
Mo4 O25 1.674(6) . ?
Mo5 Mo6 2.5879(10) . ?
Mo5 O3 2.274(6) . ?
Mo5 O6 1.975(6) . ?
Mo5 O10 2.126(6) . ?
Mo5 O16 1.946(6) . ?
Mo5 O17 2.057(6) . ?
Mo5 O24 1.679(6) . ?
Mo6 O1 2.249(6) . ?
Mo6 O6 1.966(6) . ?
Mo6 O9 2.113(6) . ?
Mo6 O15 2.062(6) . ?
Mo6 O16 1.944(6) . ?
Mo6 O23 1.673(7) . ?
Mn3 O5 2.182(6) . ?
Mn3 O5 2.182(6) 5_656 ?
Mn3 O6 2.260(6) . ?
Mn3 O6 2.260(6) 5_656 ?
Mn3 O7 2.165(6) . ?
Mn3 O7 2.165(6) 5_656 ?
Mn1 K0AA 3.047(3) 10_564 ?
Mn1 K0AA 3.989(3) 19_576 ?
Mn1 Na1 3.587(6) . ?
Mn1 O4 2.107(6) . ?
Mn1 O019 2.280(8) . ?
Mn1 O27 2.061(7) . ?
Mn1 O29 2.242(7) 19_576 ?
Mn1 O31 2.148(7) 10_564 ?
Mn1 O32 2.189(8) 10_564 ?
Mn2 O26 2.151(7) 26_556 ?
Mn2 O26 2.215(7) 10_564 ?
Mn2 O28 2.047(8) 28_656 ?
Mn2 O30 2.065(7) . ?
Mn2 O33 2.299(8) . ?
K0AA Mn1 3.047(3) 10_564 ?
K0AA P4 3.232(4) . ?
K0AA P5 3.312(2) . ?
K0AA O3 3.396(6) . ?
K0AA O4 3.080(7) . ?
K0AA O18 2.732(8) . ?
K0AA O19 2.185(6) . ?
K0AA O019 2.400(9) 28_656 ?
K0AA O29 2.162(8) 28_656 ?
K0AA O31 2.541(8) . ?
K0AA O32 2.086(8) . ?
P1 O1 1.553(6) . ?
P1 O2 1.545(6) . ?
P1 O3 1.551(6) . ?
P1 O4 1.501(6) . ?
P2 O14 1.555(6) . ?
P2 O15 1.527(6) . ?
P2 O26 1.529(6) . ?
P2 O27 1.507(7) . ?
P3 K0AA 3.480(4) 19_576 ?
P3 O11 1.550(7) . ?
P3 O12 1.531(6) . ?
P3 O28 1.520(8) . ?
P3 O29 1.508(8) . ?
P4 Na1 3.182(2) . ?
P4 O17 1.534(7) . ?
P4 O18 1.543(7) . ?
P4 O30 1.524(7) . ?
P4 O31 1.532(7) . ?
P5 K0AA 3.312(2) 19_576 ?
P5 K0AA 3.312(2) 10_564 ?
P5 K0AA 3.312(2) 28_656 ?
P5 O32 1.515(8) 19_576 ?
P5 O32 1.515(8) 28_656 ?
P5 O32 1.515(8) 10_564 ?
P5 O32 1.515(8) . ?
Na1 Mn1 3.587(6) 10_564 ?
Na1 K0AA 4.430(7) 10_564 ?
Na1 P4 3.182(2) 10_564 ?
Na1 O16 2.611(7) 10_564 ?
Na1 O16 2.611(7) . ?
Na1 O17 2.861(7) 10_564 ?
Na1 O17 2.861(7) . ?
Na1 O31 2.373(8) 10_564 ?
Na1 O31 2.373(8) . ?
O019 K0AA 2.400(9) 19_576 ?
O26 Mn2 2.151(7) 26_546 ?
O26 Mn2 2.215(7) 10_564 ?
O28 Mn2 2.047(8) 19_576 ?
O29 Mn1 2.242(7) 28_656 ?
O29 K0AA 2.162(8) 19_576 ?
O31 Mn1 2.148(7) 10_564 ?
O32 Mn1 2.189(8) 10_564 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Mo1 Mo2 87.99(15) . . ?
O5 Mo1 Mo2 48.79(17) . . ?
O5 Mo1 O1 81.0(2) . . ?
O5 Mo1 O9 86.4(2) . . ?
O5 Mo1 O14 162.4(2) . . ?
O9 Mo1 Mo2 133.82(15) . . ?
O9 Mo1 O1 72.1(2) . . ?
O13 Mo1 Mo2 48.11(17) . . ?
O13 Mo1 O1 82.6(2) . . ?
O13 Mo1 O5 95.3(2) . . ?
O13 Mo1 O9 154.1(2) . . ?
O13 Mo1 O14 89.2(3) . . ?
O14 Mo1 Mo2 137.25(19) . . ?
O14 Mo1 O1 82.8(2) . . ?
O14 Mo1 O9 82.2(2) . . ?
O22 Mo1 Mo2 100.2(2) . . ?
O22 Mo1 O1 170.9(3) . . ?
O22 Mo1 O5 101.3(3) . . ?
O22 Mo1 O9 99.2(3) . . ?
O22 Mo1 O13 105.8(3) . . ?
O22 Mo1 O14 93.7(3) . . ?
O2 Mo2 Mo1 89.63(15) . . ?
O5 Mo2 Mo1 48.65(16) . . ?
O5 Mo2 O2 81.8(2) . . ?
O5 Mo2 O8 85.7(2) . . ?
O5 Mo2 O12 160.9(2) . . ?
O8 Mo2 Mo1 133.53(17) . . ?
O8 Mo2 O2 73.3(2) . . ?
O12 Mo2 Mo1 135.16(18) . . ?
O12 Mo2 O2 79.6(2) . . ?
O12 Mo2 O8 84.8(2) . . ?
O13 Mo2 Mo1 47.79(17) . . ?
O13 Mo2 O2 84.0(2) . . ?
O13 Mo2 O5 94.8(2) . . ?
O13 Mo2 O8 157.0(2) . . ?
O13 Mo2 O12 87.6(3) . . ?
O21 Mo2 Mo1 99.8(2) . . ?
O21 Mo2 O2 170.0(3) . . ?
O21 Mo2 O5 101.7(3) . . ?
O21 Mo2 O8 97.5(3) . . ?
O21 Mo2 O12 95.9(3) . . ?
O21 Mo2 O13 104.9(3) . . ?
Mo4 Mo3 K0AA 59.35(4) . . ?
O2 Mo3 Mo4 88.36(15) . . ?
O2 Mo3 K0AA 70.02(14) . . ?
O7 Mo3 Mo4 48.97(16) . . ?
O7 Mo3 K0AA 102.42(17) . . ?
O7 Mo3 O2 81.6(2) . . ?
O7 Mo3 O8 85.8(2) . . ?
O7 Mo3 O11 161.5(2) . . ?
O8 Mo3 Mo4 133.74(17) . . ?
O8 Mo3 K0AA 140.93(16) . . ?
O8 Mo3 O2 73.7(2) . . ?
O11 Mo3 Mo4 135.24(18) . . ?
O11 Mo3 K0AA 76.18(19) . . ?
O11 Mo3 O2 80.6(2) . . ?
O11 Mo3 O8 84.3(2) . . ?
O19 Mo3 Mo4 47.70(17) . . ?
O19 Mo3 K0AA 16.15(18) . . ?
O19 Mo3 O2 82.7(2) . . ?
O19 Mo3 O7 95.1(2) . . ?
O19 Mo3 O8 156.0(2) . . ?
O19 Mo3 O11 87.7(3) . . ?
O20 Mo3 Mo4 99.7(2) . . ?
O20 Mo3 K0AA 117.1(2) . . ?
O20 Mo3 O2 171.3(3) . . ?
O20 Mo3 O7 101.0(3) . . ?
O20 Mo3 O8 98.1(3) . . ?
O20 Mo3 O11 95.9(3) . . ?
O20 Mo3 O19 105.3(3) . . ?
Mo3 Mo4 K0AA 80.48(5) . . ?
O3 Mo4 Mo3 88.56(15) . . ?
O3 Mo4 K0AA 68.95(16) . . ?
O7 Mo4 Mo3 48.54(17) . . ?
O7 Mo4 K0AA 121.10(17) . . ?
O7 Mo4 O3 80.8(2) . . ?
O7 Mo4 O10 87.7(2) . . ?
O7 Mo4 O18 160.3(3) . . ?
O10 Mo4 Mo3 135.25(17) . . ?
O10 Mo4 K0AA 126.28(17) . . ?
O10 Mo4 O3 73.2(2) . . ?
O18 Mo4 Mo3 131.9(2) . . ?
O18 Mo4 K0AA 51.7(2) . . ?
O18 Mo4 O3 79.6(2) . . ?
O18 Mo4 O10 85.4(3) . . ?
O19 Mo4 Mo3 47.95(18) . . ?
O19 Mo4 K0AA 34.77(19) . . ?
O19 Mo4 O3 83.8(2) . . ?
O19 Mo4 O7 94.9(2) . . ?
O19 Mo4 O10 156.1(2) . . ?
O19 Mo4 O18 84.3(3) . . ?
O25 Mo4 Mo3 100.0(2) . . ?
O25 Mo4 K0AA 116.7(2) . . ?
O25 Mo4 O3 170.3(3) . . ?
O25 Mo4 O7 101.4(3) . . ?
O25 Mo4 O10 97.3(3) . . ?
O25 Mo4 O18 97.7(3) . . ?
O25 Mo4 O19 105.4(3) . . ?
O3 Mo5 Mo6 87.95(15) . . ?
O6 Mo5 Mo6 48.82(16) . . ?
O6 Mo5 O3 80.4(2) . . ?
O6 Mo5 O10 86.1(2) . . ?
O6 Mo5 O17 160.2(2) . . ?
O10 Mo5 Mo6 133.69(16) . . ?
O10 Mo5 O3 72.4(2) . . ?
O16 Mo5 Mo6 48.25(17) . . ?
O16 Mo5 O3 83.5(2) . . ?
O16 Mo5 O6 95.5(2) . . ?
O16 Mo5 O10 155.2(2) . . ?
O16 Mo5 O17 86.0(3) . . ?
O17 Mo5 Mo6 133.90(18) . . ?
O17 Mo5 O3 80.2(2) . . ?
O17 Mo5 O10 84.5(2) . . ?
O24 Mo5 Mo6 101.4(2) . . ?
O24 Mo5 O3 169.4(3) . . ?
O24 Mo5 O6 101.9(3) . . ?
O24 Mo5 O10 97.4(3) . . ?
O24 Mo5 O16 106.4(3) . . ?
O24 Mo5 O17 96.5(3) . . ?
O1 Mo6 Mo5 89.99(14) . . ?
O6 Mo6 Mo5 49.10(16) . . ?
O6 Mo6 O1 82.4(2) . . ?
O6 Mo6 O9 85.0(2) . . ?
O6 Mo6 O15 160.7(2) . . ?
O9 Mo6 Mo5 133.11(15) . . ?
O9 Mo6 O1 72.6(2) . . ?
O15 Mo6 Mo5 134.42(18) . . ?
O15 Mo6 O1 78.8(2) . . ?
O15 Mo6 O9 85.5(2) . . ?
O16 Mo6 Mo5 48.34(18) . . ?
O16 Mo6 O1 84.2(2) . . ?
O16 Mo6 O6 95.9(2) . . ?
O16 Mo6 O9 156.5(2) . . ?
O16 Mo6 O15 86.4(3) . . ?
O23 Mo6 Mo5 100.6(2) . . ?
O23 Mo6 O1 168.8(3) . . ?
O23 Mo6 O6 101.8(3) . . ?
O23 Mo6 O9 97.3(3) . . ?
O23 Mo6 O15 96.0(3) . . ?
O23 Mo6 O16 105.5(3) . . ?
O5 Mn3 O5 83.6(3) 5_656 . ?
O5 Mn3 O6 96.4(2) . . ?
O5 Mn3 O6 96.4(2) 5_656 5_656 ?
O5 Mn3 O6 84.5(2) . 5_656 ?
O5 Mn3 O6 84.5(2) 5_656 . ?
O6 Mn3 O6 178.8(3) . 5_656 ?
O7 Mn3 O5 96.4(2) . . ?
O7 Mn3 O5 96.4(2) 5_656 5_656 ?
O7 Mn3 O5 178.8(2) 5_656 . ?
O7 Mn3 O5 178.8(2) . 5_656 ?
O7 Mn3 O6 96.6(2) . . ?
O7 Mn3 O6 96.6(2) 5_656 5_656 ?
O7 Mn3 O6 82.4(2) 5_656 . ?
O7 Mn3 O6 82.4(2) . 5_656 ?
O7 Mn3 O7 83.7(3) 5_656 . ?
K0AA Mn1 K0AA 92.88(6) 10_564 19_576 ?
K0AA Mn1 Na1 83.37(8) 10_564 . ?
Na1 Mn1 K0AA 133.12(10) . 19_576 ?
O4 Mn1 K0AA 124.53(18) . 10_564 ?
O4 Mn1 K0AA 81.03(19) . 19_576 ?
O4 Mn1 Na1 64.01(19) . . ?
O4 Mn1 O019 84.0(3) . . ?
O4 Mn1 O29 162.3(3) . 19_576 ?
O4 Mn1 O31 103.6(3) . 10_564 ?
O4 Mn1 O32 89.9(3) . 10_564 ?
O019 Mn1 K0AA 117.9(2) . 10_564 ?
O019 Mn1 K0AA 32.4(2) . 19_576 ?
O019 Mn1 Na1 148.01(19) . . ?
O27 Mn1 K0AA 121.6(2) . 10_564 ?
O27 Mn1 K0AA 120.3(2) . 19_576 ?
O27 Mn1 Na1 100.5(2) . . ?
O27 Mn1 O4 108.2(3) . . ?
O27 Mn1 O019 88.6(3) . . ?
O27 Mn1 O29 88.2(3) . 19_576 ?
O27 Mn1 O31 91.8(3) . 10_564 ?
O27 Mn1 O32 161.9(3) . 10_564 ?
O29 Mn1 K0AA 45.1(2) 19_576 10_564 ?
O29 Mn1 K0AA 85.1(2) 19_576 19_576 ?
O29 Mn1 Na1 120.5(2) 19_576 . ?
O29 Mn1 O019 90.2(3) 19_576 . ?
O31 Mn1 K0AA 144.8(2) 10_564 19_576 ?
O31 Mn1 K0AA 55.4(2) 10_564 10_564 ?
O31 Mn1 Na1 39.8(2) 10_564 . ?
O31 Mn1 O019 171.8(3) 10_564 . ?
O31 Mn1 O29 81.7(3) 10_564 19_576 ?
O31 Mn1 O32 84.8(3) 10_564 10_564 ?
O32 Mn1 K0AA 43.2(2) 10_564 10_564 ?
O32 Mn1 K0AA 60.2(2) 10_564 19_576 ?
O32 Mn1 Na1 88.2(3) 10_564 . ?
O32 Mn1 O019 92.3(3) 10_564 . ?
O32 Mn1 O29 73.7(3) 10_564 19_576 ?
O26 Mn2 O26 77.5(3) 26_556 10_564 ?
O26 Mn2 O33 145.9(3) 10_564 . ?
O26 Mn2 O33 81.8(3) 26_556 . ?
O28 Mn2 O26 99.2(3) 28_656 26_556 ?
O28 Mn2 O26 113.1(3) 28_656 10_564 ?
O28 Mn2 O30 122.7(3) 28_656 . ?
O28 Mn2 O33 96.7(3) 28_656 . ?
O30 Mn2 O26 93.2(3) . 10_564 ?
O30 Mn2 O26 136.9(3) . 26_556 ?
O30 Mn2 O33 83.6(3) . . ?
Mn1 K0AA Mo4 125.07(9) 10_564 . ?
Mn1 K0AA P4 65.68(7) 10_564 . ?
Mn1 K0AA P5 64.94(5) 10_564 . ?
Mn1 K0AA O3 106.97(13) 10_564 . ?
Mn1 K0AA O4 92.71(14) 10_564 . ?
P4 K0AA Mo4 59.39(6) . . ?
P4 K0AA P5 118.10(9) . . ?
P4 K0AA O3 55.18(11) . . ?
P5 K0AA Mo4 145.62(9) . . ?
P5 K0AA O3 109.38(12) . . ?
O3 K0AA Mo4 38.17(10) . . ?
O4 K0AA Mo4 81.17(12) . . ?
O4 K0AA P4 82.78(15) . . ?
O4 K0AA P5 64.91(12) . . ?
O4 K0AA O3 44.83(15) . . ?
O18 K0AA Mo4 35.71(14) . . ?
O18 K0AA Mn1 91.28(16) . 10_564 ?
O18 K0AA P4 28.42(15) . . ?
O18 K0AA P5 145.54(18) . . ?
O18 K0AA O3 51.83(17) . . ?
O18 K0AA O4 93.5(2) . . ?
O19 K0AA Mo4 30.38(16) . . ?
O19 K0AA Mn1 155.4(2) . 10_564 ?
O19 K0AA P4 89.76(18) . . ?
O19 K0AA P5 133.70(18) . . ?
O19 K0AA O3 55.33(19) . . ?
O19 K0AA O4 84.9(2) . . ?
O19 K0AA O18 64.5(2) . . ?
O19 K0AA O019 74.1(2) . 28_656 ?
O19 K0AA O31 112.9(2) . . ?
O019 K0AA Mo4 103.45(19) 28_656 . ?
O019 K0AA Mn1 128.8(2) 28_656 10_564 ?
O019 K0AA P4 156.8(2) 28_656 . ?
O019 K0AA P5 85.01(19) 28_656 . ?
O019 K0AA O3 122.3(2) 28_656 . ?
O019 K0AA O4 111.6(2) 28_656 . ?
O019 K0AA O18 129.1(2) 28_656 . ?
O019 K0AA O31 172.8(3) 28_656 . ?
O29 K0AA Mo4 115.9(2) 28_656 . ?
O29 K0AA Mn1 47.3(2) 28_656 10_564 ?
O29 K0AA P4 77.1(2) 28_656 . ?
O29 K0AA P5 94.8(2) 28_656 . ?
O29 K0AA O3 132.1(3) 28_656 . ?
O29 K0AA O4 139.8(2) 28_656 . ?
O29 K0AA O18 85.0(3) 28_656 . ?
O29 K0AA O19 128.8(3) 28_656 . ?
O29 K0AA O019 99.9(3) 28_656 28_656 ?
O29 K0AA O31 74.8(3) 28_656 . ?
O31 K0AA Mo4 83.32(16) . . ?
O31 K0AA Mn1 44.06(16) . 10_564 ?
O31 K0AA P4 27.59(16) . . ?
O31 K0AA P5 90.67(17) . . ?
O31 K0AA O3 64.60(18) . . ?
O31 K0AA O4 71.4(2) . . ?
O31 K0AA O18 55.9(2) . . ?
O32 K0AA Mo4 153.1(3) . . ?
O32 K0AA Mn1 45.9(2) . 10_564 ?
O32 K0AA P4 105.0(2) . . ?
O32 K0AA P5 19.5(2) . . ?
O32 K0AA O3 115.2(3) . . ?
O32 K0AA O4 74.8(3) . . ?
O32 K0AA O18 133.4(3) . . ?
O32 K0AA O19 152.8(3) . . ?
O32 K0AA O019 96.6(3) . 28_656 ?
O32 K0AA O29 77.4(3) . 28_656 ?
O32 K0AA O31 77.7(3) . . ?
O1 P1 K0AA 165.1(2) . . ?
O2 P1 K0AA 87.1(2) . . ?
O2 P1 O1 107.5(3) . . ?
O2 P1 O3 106.9(3) . . ?
O3 P1 K0AA 69.4(2) . . ?
O3 P1 O1 107.7(3) . . ?
O4 P1 K0AA 57.5(3) . . ?
O4 P1 O1 112.3(4) . . ?
O4 P1 O2 113.1(4) . . ?
O4 P1 O3 109.1(3) . . ?
O15 P2 O14 109.1(4) . . ?
O15 P2 O26 109.2(4) . . ?
O26 P2 O14 108.6(4) . . ?
O27 P2 O14 108.9(4) . . ?
O27 P2 O15 114.2(4) . . ?
O27 P2 O26 106.8(4) . . ?
O11 P3 K0AA 122.6(3) . 19_576 ?
O12 P3 K0AA 87.5(3) . 19_576 ?
O12 P3 O11 110.5(4) . . ?
O28 P3 K0AA 115.5(3) . 19_576 ?
O28 P3 O11 109.4(4) . . ?
O28 P3 O12 108.4(4) . . ?
O29 P3 K0AA 22.3(3) . 19_576 ?
O29 P3 O11 108.6(4) . . ?
O29 P3 O12 109.3(4) . . ?
O29 P3 O28 110.5(5) . . ?
Na1 P4 K0AA 87.35(16) . . ?
O17 P4 K0AA 127.5(3) . . ?
O17 P4 Na1 63.9(3) . . ?
O17 P4 O18 110.4(4) . . ?
O18 P4 K0AA 57.5(3) . . ?
O18 P4 Na1 132.1(3) . . ?
O30 P4 K0AA 125.0(3) . . ?
O30 P4 Na1 117.6(3) . . ?
O30 P4 O17 107.3(4) . . ?
O30 P4 O18 109.5(4) . . ?
O30 P4 O31 113.9(4) . . ?
O31 P4 K0AA 50.2(3) . . ?
O31 P4 Na1 45.4(3) . . ?
O31 P4 O17 108.2(4) . . ?
O31 P4 O18 107.5(4) . . ?
K0AA P5 K0AA 126.27(9) 10_564 . ?
K0AA P5 K0AA 101.78(4) 28_656 . ?
K0AA P5 K0AA 101.78(4) 10_564 28_656 ?
K0AA P5 K0AA 101.78(4) 10_564 19_576 ?
K0AA P5 K0AA 101.78(4) 19_576 . ?
K0AA P5 K0AA 126.27(9) 19_576 28_656 ?
O32 P5 K0AA 27.3(3) 10_564 10_564 ?
O32 P5 K0AA 112.5(3) 19_576 28_656 ?
O32 P5 K0AA 112.5(3) 28_656 19_576 ?
O32 P5 K0AA 129.1(3) 28_656 . ?
O32 P5 K0AA 129.1(3) 19_576 10_564 ?
O32 P5 K0AA 27.3(3) 19_576 19_576 ?
O32 P5 K0AA 82.8(4) 19_576 . ?
O32 P5 K0AA 82.8(4) . 28_656 ?
O32 P5 K0AA 82.8(4) 28_656 10_564 ?
O32 P5 K0AA 112.5(3) . 10_564 ?
O32 P5 K0AA 129.1(3) . 19_576 ?
O32 P5 K0AA 27.3(3) . . ?
O32 P5 K0AA 82.8(4) 10_564 19_576 ?
O32 P5 K0AA 129.1(3) 10_564 28_656 ?
O32 P5 K0AA 112.5(3) 10_564 . ?
O32 P5 K0AA 27.3(3) 28_656 28_656 ?
O32 P5 O32 108.3(3) 28_656 10_564 ?
O32 P5 O32 111.9(7) . 10_564 ?
O32 P5 O32 108.3(3) . 19_576 ?
O32 P5 O32 108.3(3) . 28_656 ?
O32 P5 O32 108.3(3) 10_564 19_576 ?
O32 P5 O32 111.9(7) 28_656 19_576 ?
Mn1 Na1 Mn1 90.76(19) 10_564 . ?
Mn1 Na1 K0AA 43.10(8) . 10_564 ?
Mn1 Na1 K0AA 71.55(13) 10_564 10_564 ?
Mn1 Na1 K0AA 71.55(13) . . ?
Mn1 Na1 K0AA 43.10(8) 10_564 . ?
K0AA Na1 K0AA 83.67(15) 10_564 . ?
P4 Na1 Mn1 115.01(18) . . ?
P4 Na1 Mn1 115.02(18) 10_564 10_564 ?
P4 Na1 Mn1 60.13(8) 10_564 . ?
P4 Na1 Mn1 60.12(8) . 10_564 ?
P4 Na1 K0AA 46.80(9) 10_564 10_564 ?
P4 Na1 K0AA 127.2(2) . 10_564 ?
P4 Na1 K0AA 127.2(2) 10_564 . ?
P4 Na1 K0AA 46.79(9) . . ?
P4 Na1 P4 173.9(3) . 10_564 ?
O16 Na1 Mn1 85.06(15) . . ?
O16 Na1 Mn1 85.06(15) 10_564 10_564 ?
O16 Na1 Mn1 138.27(17) 10_564 . ?
O16 Na1 Mn1 138.27(17) . 10_564 ?
O16 Na1 K0AA 125.25(17) . 10_564 ?
O16 Na1 K0AA 97.07(16) 10_564 10_564 ?
O16 Na1 K0AA 125.26(17) 10_564 . ?
O16 Na1 K0AA 97.07(16) . . ?
O16 Na1 P4 98.62(16) . 10_564 ?
O16 Na1 P4 84.29(15) 10_564 10_564 ?
O16 Na1 P4 84.29(15) . . ?
O16 Na1 P4 98.62(16) 10_564 . ?
O16 Na1 O16 123.9(4) . 10_564 ?
O16 Na1 O17 59.67(19) . . ?
O16 Na1 O17 99.6(2) 10_564 . ?
O16 Na1 O17 59.67(19) 10_564 10_564 ?
O16 Na1 O17 99.6(2) . 10_564 ?
O17 Na1 Mn1 121.86(16) 10_564 10_564 ?
O17 Na1 Mn1 88.74(14) . 10_564 ?
O17 Na1 Mn1 88.75(14) 10_564 . ?
O17 Na1 Mn1 121.86(16) . . ?
O17 Na1 K0AA 69.29(15) 10_564 10_564 ?
O17 Na1 K0AA 152.9(3) . 10_564 ?
O17 Na1 K0AA 152.9(3) 10_564 . ?
O17 Na1 K0AA 69.28(15) . . ?
O17 Na1 P4 156.2(3) . 10_564 ?
O17 Na1 P4 156.2(3) 10_564 . ?
O17 Na1 P4 28.78(13) 10_564 10_564 ?
O17 Na1 P4 28.78(13) . . ?
O17 Na1 O17 137.8(4) 10_564 . ?
O31 Na1 Mn1 97.8(3) . . ?
O31 Na1 Mn1 35.37(18) 10_564 . ?
O31 Na1 Mn1 35.37(18) . 10_564 ?
O31 Na1 Mn1 97.8(3) 10_564 10_564 ?
O31 Na1 K0AA 26.6(2) . . ?
O31 Na1 K0AA 100.0(3) 10_564 . ?
O31 Na1 K0AA 26.6(2) 10_564 10_564 ?
O31 Na1 K0AA 100.0(3) . 10_564 ?
O31 Na1 P4 146.7(3) 10_564 . ?
O31 Na1 P4 27.37(17) 10_564 10_564 ?
O31 Na1 P4 146.7(3) . 10_564 ?
O31 Na1 P4 27.37(17) . . ?
O31 Na1 O16 102.2(2) 10_564 . ?
O31 Na1 O16 102.2(2) . 10_564 ?
O31 Na1 O16 104.1(2) 10_564 10_564 ?
O31 Na1 O16 104.1(2) . . ?
O31 Na1 O17 155.8(2) . 10_564 ?
O31 Na1 O17 155.8(2) 10_564 . ?
O31 Na1 O17 55.7(2) 10_564 10_564 ?
O31 Na1 O17 55.7(2) . . ?
O31 Na1 O31 122.1(5) 10_564 . ?
Mo6 O1 Mo1 101.1(2) . . ?
P1 O1 Mo1 127.2(3) . . ?
P1 O1 Mo6 125.3(3) . . ?
Mo2 O2 Mo3 99.4(2) . . ?
P1 O2 Mo2 126.2(3) . . ?
P1 O2 Mo3 126.7(3) . . ?
Mo4 O3 Mo5 101.6(2) . . ?
Mo4 O3 K0AA 72.88(16) . . ?
Mo5 O3 K0AA 135.0(2) . . ?
P1 O3 Mo4 127.6(3) . . ?
P1 O3 Mo5 126.1(3) . . ?
P1 O3 K0AA 85.3(2) . . ?
Mn1 O4 K0AA 130.9(3) . . ?
P1 O4 Mn1 130.7(4) . . ?
P1 O4 K0AA 98.3(3) . . ?
Mo1 O5 Mo2 82.6(2) . . ?
Mo1 O5 Mn3 134.0(3) . . ?
Mo2 O5 Mn3 134.0(3) . . ?
Mo5 O6 Mn3 133.3(3) . . ?
Mo6 O6 Mo5 82.1(2) . . ?
Mo6 O6 Mn3 132.9(3) . . ?
Mo3 O7 Mo4 82.5(2) . . ?
Mo3 O7 Mn3 134.3(3) . . ?
Mo4 O7 Mn3 133.5(3) . . ?
Mo3 O8 Mo2 112.9(3) . . ?
Mo1 O9 Mo6 113.1(3) . . ?
Mo4 O10 Mo5 111.8(3) . . ?
P3 O11 Mo3 137.8(4) . . ?
P3 O12 Mo2 138.4(4) . . ?
Mo1 O13 Mo2 84.1(2) . . ?
P2 O14 Mo1 130.5(4) . . ?
P2 O15 Mo6 135.0(4) . . ?
Mo5 O16 Na1 112.3(3) . . ?
Mo6 O16 Mo5 83.4(2) . . ?
Mo6 O16 Na1 155.7(3) . . ?
Mo5 O17 Na1 100.0(2) . . ?
P4 O17 Mo5 135.9(4) . . ?
P4 O17 Na1 87.3(3) . . ?
Mo4 O18 K0AA 92.6(3) . . ?
P4 O18 Mo4 137.0(4) . . ?
P4 O18 K0AA 94.1(3) . . ?
Mo3 O19 K0AA 149.5(3) . . ?
Mo4 O19 Mo3 84.3(2) . . ?
Mo4 O19 K0AA 114.8(3) . . ?
Mn1 O019 K0AA 117.0(3) . 19_576 ?
Mn2 O26 Mn2 102.5(3) 26_546 10_564 ?
P2 O26 Mn2 108.9(4) . 10_564 ?
P2 O26 Mn2 146.2(4) . 26_546 ?
P2 O27 Mn1 151.8(5) . . ?
P3 O28 Mn2 135.3(5) . 19_576 ?
K0AA O29 Mn1 87.6(3) 19_576 28_656 ?
P3 O29 Mn1 130.1(4) . 28_656 ?
P3 O29 K0AA 142.4(5) . 19_576 ?
P4 O30 Mn2 131.8(4) . . ?
Mn1 O31 K0AA 80.6(2) 10_564 . ?
Mn1 O31 Na1 104.9(3) 10_564 . ?
P4 O31 Mn1 135.1(4) . 10_564 ?
P4 O31 K0AA 102.2(4) . . ?
P4 O31 Na1 107.2(4) . . ?
Na1 O31 K0AA 128.7(3) . . ?
K0AA O32 Mn1 90.9(3) . 10_564 ?
P5 O32 Mn1 134.2(5) . 10_564 ?
P5 O32 K0AA 133.2(5) . . ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_NENU_606
_database_code_depnum_ccdc_archive 'CCDC 1855994'
_audit_update_record             
;
2018-07-16 deposited with the CCDC.
2018-10-01 downloaded from the CCDC.
;
_audit_creation_date             2018-07-13
_audit_creation_method           
;
Olex2 1.2
(compiled 2017.03.28 svn.r3405 for OlexSys, GUI svn.r5370)
;
_shelx_SHELXL_version_number     2016/4
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         '0.5(Co20 Mn60 Mo192 Na48 O1056 P136), 48(O)'
_chemical_formula_sum            'Co10 Mn30 Mo96 Na24 O576 P68'
_chemical_formula_weight         23321.46
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      tetragonal
_space_group_IT_number           142
_space_group_name_H-M_alt        'I 41/a c d'
_space_group_name_Hall           '-I 4bd 2c'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-y+1/4, x+3/4, z+1/4'
'y+1/4, -x+1/4, z+3/4'
'-x+1/2, y, -z'
'x, -y, -z+1/2'
'y+1/4, x+3/4, -z+3/4'
'-y+1/4, -x+1/4, -z+1/4'
'x+1/2, y+1/2, z+1/2'
'-x+1, -y+1/2, z+1'
'-y+3/4, x+5/4, z+3/4'
'y+3/4, -x+3/4, z+5/4'
'-x+1, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1'
'y+3/4, x+5/4, -z+5/4'
'-y+3/4, -x+3/4, -z+3/4'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'y-1/4, -x-3/4, -z-1/4'
'-y-1/4, x-1/4, -z-3/4'
'x-1/2, -y, z'
'-x, y, z-1/2'
'-y-1/4, -x-3/4, z-3/4'
'y-1/4, x-1/4, z-1/4'
'-x+1/2, -y+1/2, -z+1/2'
'x, y+1/2, -z'
'y+1/4, -x-1/4, -z+1/4'
'-y+1/4, x+1/4, -z-1/4'
'x, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z'
'-y+1/4, -x-1/4, z-1/4'
'y+1/4, x+1/4, z+1/4'

_cell_length_a                   26.9679(5)
_cell_length_b                   26.9679(5)
_cell_length_c                   41.1540(18)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     29930.0(17)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    9190
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.465
_cell_measurement_theta_min      2.248
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    3.128
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_correction_T_min  0.7094
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
'SADABS-2014/5 (Bruker,2014/5) was used for absorption correction. wR2(int) was 0.0561 before and 0.0450 after correction. The Ratio of minimum to maximum transmission is 0.9514. The λ/2 correction factor is Not present.'
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'clear reddish red'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   reddish
_exptl_crystal_colour_primary    red
_exptl_crystal_density_diffrn    2.588
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       octahedral
_exptl_crystal_F_000             21888
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.2
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0348
_diffrn_reflns_av_unetI/netI     0.0194
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -31
_diffrn_reflns_limit_k_max       35
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       53
_diffrn_reflns_limit_l_min       -53
_diffrn_reflns_number            83160
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.502
_diffrn_reflns_theta_min         2.768
_diffrn_ambient_temperature      293.0
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  CMOS-PHOTON100
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                7411
_reflns_number_total             8600
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT v8.37A (Bruker, 2015)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT v8.37A (Bruker, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'olex2.solve (Bourhis et al., 2015)'
_refine_diff_density_max         1.511
_refine_diff_density_min         -1.148
_refine_diff_density_rms         0.134
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.041
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     455
_refine_ls_number_reflns         8600
_refine_ls_number_restraints     12
_refine_ls_R_factor_all          0.0400
_refine_ls_R_factor_gt           0.0316
_refine_ls_restrained_S_all      1.050
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0286P)²+400.1517P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0736
_refine_ls_wR_factor_ref         0.0768
_refine_special_details          ?
_olex2_refinement_description    
;
1. Shared sites
{Mn3, Co3}
{Mn1, Co1}
{Mn2, Co2}
2. Uiso/Uaniso restraints and constraints
P5 \\sim O32: within 1.7A with sigma of 0.01 and sigma for terminal atoms of
0.02
Uanis(O32) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.2
Uanis(Mn3) = Uanis(Co3)
Uanis(Mn1) = Uanis(Co1)
Uanis(Mn2) = Uanis(Co2)
3. Others
 Fixed Sof: Mn3(0.375) Mn1(0.75) Mn2(0.75) Co3(0.125) Co1(0.25) Co2(0.25)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     iterative
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.52244(2) 0.52274(2) 0.33101(2) 0.01368(8) Uani 1 1 d . . . . .
Mo2 Mo 0.56968(2) 0.56664(2) 0.28432(2) 0.01410(8) Uani 1 1 d . . . . .
Mo3 Mo 0.50571(2) 0.62638(2) 0.22181(2) 0.01488(8) Uani 1 1 d . . . . .
Mo4 Mo 0.40961(2) 0.62627(2) 0.22234(2) 0.01502(8) Uani 1 1 d . . . . .
Mo5 Mo 0.34409(2) 0.56566(2) 0.28433(2) 0.01415(8) Uani 1 1 d . . . . .
Mo6 Mo 0.39359(2) 0.52566(2) 0.33172(2) 0.01390(8) Uani 1 1 d . . . . .
Mn3 Mn 0.45709(3) 0.500000 0.250000 0.01168(16) Uani 0.75 2 d S T P . .
Mn1 Mn 0.39974(3) 0.72784(3) 0.31961(2) 0.03110(18) Uani 0.75 1 d . . . . .
Mn2 Mn 0.29176(3) 0.78387(4) 0.27593(2) 0.0348(2) Uani 0.75 1 d . . . . .
Co3 Co 0.45709(3) 0.500000 0.250000 0.01168(16) Uani 0.25 2 d S T P . .
Co1 Co 0.39974(3) 0.72784(3) 0.31961(2) 0.03110(18) Uani 0.25 1 d . . . . .
Co2 Co 0.29176(3) 0.78387(4) 0.27593(2) 0.0348(2) Uani 0.25 1 d . . . . .
P1 P 0.45691(4) 0.62289(4) 0.29846(3) 0.0126(2) Uani 1 1 d . . . . .
P2 P 0.45971(4) 0.55317(5) 0.39853(3) 0.0215(2) Uani 1 1 d . . . . .
P3 P 0.59576(4) 0.68351(4) 0.26306(3) 0.0185(2) Uani 1 1 d . . . . .
P4 P 0.31744(5) 0.68013(4) 0.26259(3) 0.0233(3) Uani 1 1 d . . . . .
P5 P 0.500000 0.750000 0.375000 0.0820(14) Uani 1 4 d S TU P . .
Na1 Na 0.500000 0.750000 0.26225(11) 0.0602(10) Uani 1 2 d S T P . .
Na2 Na 0.57722(15) 0.66284(10) 0.34251(8) 0.0773(11) Uani 1 1 d . . . . .
O1 O 0.50345(11) 0.61751(11) 0.27670(7) 0.0160(6) Uani 1 1 d . . . . .
O2 O 0.41024(11) 0.61689(11) 0.27670(7) 0.0157(6) Uani 1 1 d . . . . .
O3 O 0.45660(12) 0.67269(11) 0.31481(8) 0.0238(7) Uani 1 1 d . . . . .
O4 O 0.45766(10) 0.57842(11) 0.32229(7) 0.0151(6) Uani 1 1 d . . . . .
O5 O 0.55988(11) 0.57340(11) 0.23391(7) 0.0181(6) Uani 1 1 d . . . . .
O6 O 0.35532(11) 0.57256(11) 0.23410(7) 0.0165(6) Uani 1 1 d . . . . .
O7 O 0.45754(11) 0.48085(10) 0.33332(7) 0.0158(6) Uani 1 1 d . . . . .
O8 O 0.51620(11) 0.51658(11) 0.28336(7) 0.0146(6) Uani 1 1 d . . . . .
O9 O 0.45774(11) 0.57113(10) 0.22508(7) 0.0148(6) Uani 1 1 d . . . . .
O10 O 0.39838(11) 0.51675(10) 0.28417(7) 0.0143(6) Uani 1 1 d . . . . .
O11 O 0.35285(11) 0.58491(11) 0.32960(7) 0.0189(6) Uani 1 1 d . . . . .
O12 O 0.56177(11) 0.58287(11) 0.32987(7) 0.0184(6) Uani 1 1 d . . . . .
O13 O 0.45785(12) 0.67857(11) 0.23049(7) 0.0197(6) Uani 1 1 d . . . . .
O14 O 0.35488(12) 0.67509(12) 0.23501(8) 0.0231(7) Uani 1 1 d . . . . .
O15 O 0.30523(12) 0.63001(12) 0.27802(8) 0.0239(7) Uani 1 1 d . . . . .
O16 O 0.41235(12) 0.54581(12) 0.37807(7) 0.0224(7) Uani 1 1 d . . . . .
O17 O 0.50624(11) 0.54041(12) 0.37823(7) 0.0210(7) Uani 1 1 d . . . . .
O18 O 0.60365(12) 0.63372(11) 0.28143(8) 0.0229(7) Uani 1 1 d . . . . .
O19 O 0.55950(12) 0.67647(12) 0.23428(8) 0.0242(7) Uani 1 1 d . . . . .
O20 O 0.29411(12) 0.52849(12) 0.28377(8) 0.0239(7) Uani 1 1 d . . . . .
O21 O 0.35428(12) 0.48022(12) 0.34218(8) 0.0244(7) Uani 1 1 d . . . . .
O22 O 0.56269(12) 0.47735(12) 0.33951(8) 0.0228(7) Uani 1 1 d . . . . .
O23 O 0.62103(12) 0.53131(13) 0.28262(8) 0.0245(7) Uani 1 1 d . . . . .
O24 O 0.51664(13) 0.62850(13) 0.18177(8) 0.0265(7) Uani 1 1 d . . . . .
O25 O 0.39802(13) 0.62807(12) 0.18224(8) 0.0262(7) Uani 1 1 d . . . . .
O26 O 0.45807(16) 0.51877(19) 0.42749(9) 0.0509(12) Uani 1 1 d . . . . .
O27 O 0.46331(14) 0.60627(17) 0.40943(12) 0.0521(13) Uani 1 1 d . . . . .
O28 O 0.57289(12) 0.72086(12) 0.28596(9) 0.0271(8) Uani 1 1 d . . . . .
O29 O 0.64593(12) 0.69857(13) 0.24971(9) 0.0289(8) Uani 1 1 d . . . . .
O30 O 0.27209(17) 0.7053(2) 0.25028(13) 0.0705(17) Uani 1 1 d . . . . .
O31 O 0.3370(2) 0.71377(15) 0.28925(10) 0.0572(14) Uani 1 1 d . . . . .
O32 O 0.5446(3) 0.7371(3) 0.35424(18) 0.120(2) Uani 1 1 d . U . . .
O33 O 0.57390(13) 0.61874(15) 0.39460(9) 0.0359(9) Uani 1 1 d . . . . .
O1W O 0.250000 0.5425(2) 0.500000 0.088(3) Uani 1 2 d S T P . .
O2W O 0.3696(4) 0.5395(3) 0.4754(3) 0.166(4) Uani 1 1 d . . . . .
O3W O 0.3574(3) 0.4643(3) 0.4238(2) 0.121(3) Uani 1 1 d . . . . .
O4W O 0.34899(17) 0.59899(17) 0.125000 0.0483(15) Uani 1 2 d S T P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 Mo2 2.5915(5) . ?
Mo1 O4 2.331(3) . ?
Mo1 O7 2.085(3) . ?
Mo1 O8 1.975(3) . ?
Mo1 O12 1.938(3) . ?
Mo1 O17 2.048(3) . ?
Mo1 O22 1.673(3) . ?
Mo2 Na2 3.537(3) . ?
Mo2 O1 2.274(3) . ?
Mo2 O5 2.100(3) . ?
Mo2 O8 1.976(3) . ?
Mo2 O12 1.937(3) . ?
Mo2 O18 2.031(3) . ?
Mo2 O23 1.682(3) . ?
Mo3 Mo4 2.5916(5) . ?
Mo3 O1 2.272(3) . ?
Mo3 O5 2.103(3) . ?
Mo3 O9 1.978(3) . ?
Mo3 O13 1.943(3) . ?
Mo3 O19 2.047(3) . ?
Mo3 O24 1.675(3) . ?
Mo4 O2 2.252(3) . ?
Mo4 O6 2.116(3) . ?
Mo4 O9 1.977(3) . ?
Mo4 O13 1.948(3) . ?
Mo4 O14 2.045(3) . ?
Mo4 O25 1.680(3) . ?
Mo5 Mo6 2.5979(5) . ?
Mo5 O2 2.278(3) . ?
Mo5 O6 2.098(3) . ?
Mo5 O10 1.971(3) . ?
Mo5 O11 1.948(3) . ?
Mo5 O15 2.044(3) . ?
Mo5 O20 1.680(3) . ?
Mo6 O4 2.272(3) . ?
Mo6 O7 2.107(3) . ?
Mo6 O10 1.976(3) . ?
Mo6 O11 1.941(3) . ?
Mo6 O16 2.047(3) . ?
Mo6 O21 1.677(3) . ?
Mn3 O8 2.151(3) 6_565 ?
Mn3 O8 2.151(3) . ?
Mn3 O9 2.175(3) . ?
Mn3 O9 2.175(3) 6_565 ?
Mn3 O10 2.165(3) 6_565 ?
Mn3 O10 2.165(3) . ?
Mn1 Na1 3.638(3) . ?
Mn1 Na2 3.157(3) 10_564 ?
Mn1 O3 2.145(3) . ?
Mn1 O27 2.154(4) 19_576 ?
Mn1 O28 2.092(3) 10_564 ?
Mn1 O31 2.137(6) . ?
Mn1 O32 2.276(7) 10_564 ?
Mn1 O33 2.194(4) 19_576 ?
Mn2 P4 2.9340(15) . ?
Mn2 O26 2.026(4) 19_576 ?
Mn2 O29 2.052(4) 10_564 ?
Mn2 O30 2.053(5) 25_565 ?
Mn2 O30 2.426(7) . ?
Mn2 O31 2.316(5) . ?
P1 O1 1.549(3) . ?
P1 O2 1.553(3) . ?
P1 O3 1.502(3) . ?
P1 O4 1.550(3) . ?
P2 O16 1.543(3) . ?
P2 O17 1.546(3) . ?
P2 O26 1.511(4) . ?
P2 O27 1.504(4) . ?
P3 Na1 3.1441(12) . ?
P3 Na2 3.354(3) . ?
P3 O18 1.556(3) . ?
P3 O19 1.548(3) . ?
P3 O28 1.511(3) . ?
P3 O29 1.516(3) . ?
P4 O14 1.525(3) . ?
P4 O15 1.529(3) . ?
P4 O30 1.488(4) . ?
P4 O31 1.518(4) . ?
P5 Na2 3.413(3) 19_576 ?
P5 Na2 3.413(3) . ?
P5 Na2 3.413(3) 28_656 ?
P5 Na2 3.413(3) 10_564 ?
P5 O32 1.517(7) 28_656 ?
P5 O32 1.517(7) 19_576 ?
P5 O32 1.517(7) . ?
P5 O32 1.517(7) 10_564 ?
Na1 Mn1 3.639(3) 10_564 ?
Na1 P3 3.1440(12) 10_564 ?
Na1 O13 2.591(4) . ?
Na1 O13 2.591(4) 10_564 ?
Na1 O19 2.798(4) 10_564 ?
Na1 O19 2.798(4) . ?
Na1 O28 2.331(4) 10_564 ?
Na1 O28 2.331(4) . ?
Na2 Mn1 3.157(3) 10_564 ?
Na2 Co1 3.157(3) 10_564 ?
Na2 O12 2.257(4) . ?
Na2 O18 2.728(4) . ?
Na2 O27 2.253(5) 28_656 ?
Na2 O28 2.807(5) . ?
Na2 O32 2.239(8) . ?
Na2 O33 2.453(5) . ?
O26 Mn2 2.026(4) 28_656 ?
O26 Co2 2.026(4) 28_656 ?
O27 Mn1 2.154(4) 28_656 ?
O27 Co1 2.154(4) 28_656 ?
O27 Na2 2.253(5) 19_576 ?
O28 Mn1 2.092(3) 10_564 ?
O28 Co1 2.092(3) 10_564 ?
O29 Mn2 2.053(4) 10_564 ?
O29 Co2 2.053(4) 10_564 ?
O30 Mn2 2.053(5) 25_565 ?
O30 Co2 2.053(5) 25_565 ?
O32 Mn1 2.276(7) 10_564 ?
O32 Co1 2.276(7) 10_564 ?
O33 Mn1 2.194(4) 28_656 ?
O33 Co1 2.194(4) 28_656 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O4 Mo1 Mo2 87.71(7) . . ?
O7 Mo1 Mo2 133.93(8) . . ?
O7 Mo1 O4 74.15(11) . . ?
O8 Mo1 Mo2 49.02(8) . . ?
O8 Mo1 O4 80.65(11) . . ?
O8 Mo1 O7 85.88(12) . . ?
O8 Mo1 O17 160.64(12) . . ?
O12 Mo1 Mo2 48.00(9) . . ?
O12 Mo1 O4 82.38(12) . . ?
O12 Mo1 O7 156.01(12) . . ?
O12 Mo1 O8 95.34(12) . . ?
O12 Mo1 O17 86.84(13) . . ?
O17 Mo1 Mo2 134.59(9) . . ?
O17 Mo1 O4 80.58(11) . . ?
O17 Mo1 O7 84.48(12) . . ?
O22 Mo1 Mo2 99.80(11) . . ?
O22 Mo1 O4 171.73(14) . . ?
O22 Mo1 O7 97.98(14) . . ?
O22 Mo1 O8 101.61(14) . . ?
O22 Mo1 O12 105.20(15) . . ?
O22 Mo1 O17 96.33(14) . . ?
Mo1 Mo2 Na2 82.03(5) . . ?
O1 Mo2 Mo1 89.53(7) . . ?
O1 Mo2 Na2 72.30(10) . . ?
O5 Mo2 Mo1 135.27(9) . . ?
O5 Mo2 Na2 127.78(10) . . ?
O5 Mo2 O1 73.28(11) . . ?
O8 Mo2 Mo1 49.00(8) . . ?
O8 Mo2 Na2 123.84(10) . . ?
O8 Mo2 O1 80.56(11) . . ?
O8 Mo2 O5 87.00(12) . . ?
O8 Mo2 O18 159.48(13) . . ?
O12 Mo2 Mo1 48.05(9) . . ?
O12 Mo2 Na2 35.43(10) . . ?
O12 Mo2 O1 84.88(12) . . ?
O12 Mo2 O5 157.37(13) . . ?
O12 Mo2 O8 95.36(12) . . ?
O12 Mo2 O18 84.56(13) . . ?
O18 Mo2 Mo1 132.22(10) . . ?
O18 Mo2 Na2 50.24(10) . . ?
O18 Mo2 O1 78.99(12) . . ?
O18 Mo2 O5 85.50(12) . . ?
O23 Mo2 Mo1 100.19(12) . . ?
O23 Mo2 Na2 113.35(13) . . ?
O23 Mo2 O1 169.25(14) . . ?
O23 Mo2 O5 96.41(14) . . ?
O23 Mo2 O8 102.30(14) . . ?
O23 Mo2 O12 105.01(15) . . ?
O23 Mo2 O18 97.51(15) . . ?
O1 Mo3 Mo4 87.98(8) . . ?
O5 Mo3 Mo4 133.77(9) . . ?
O5 Mo3 O1 73.25(11) . . ?
O9 Mo3 Mo4 49.05(8) . . ?
O9 Mo3 O1 80.52(11) . . ?
O9 Mo3 O5 85.78(12) . . ?
O9 Mo3 O19 160.62(12) . . ?
O13 Mo3 Mo4 48.31(9) . . ?
O13 Mo3 O1 82.86(12) . . ?
O13 Mo3 O5 155.52(12) . . ?
O13 Mo3 O9 95.67(12) . . ?
O13 Mo3 O19 86.94(13) . . ?
O19 Mo3 Mo4 135.00(10) . . ?
O19 Mo3 O1 80.75(12) . . ?
O19 Mo3 O5 84.08(13) . . ?
O24 Mo3 Mo4 100.62(12) . . ?
O24 Mo3 O1 170.50(14) . . ?
O24 Mo3 O5 97.69(15) . . ?
O24 Mo3 O9 101.99(14) . . ?
O24 Mo3 O13 105.85(15) . . ?
O24 Mo3 O19 95.71(15) . . ?
O2 Mo4 Mo3 90.06(8) . . ?
O6 Mo4 Mo3 134.00(8) . . ?
O6 Mo4 O2 72.60(11) . . ?
O9 Mo4 Mo3 49.07(8) . . ?
O9 Mo4 O2 81.59(11) . . ?
O9 Mo4 O6 85.77(11) . . ?
O9 Mo4 O14 160.62(12) . . ?
O13 Mo4 Mo3 48.15(9) . . ?
O13 Mo4 O2 84.56(12) . . ?
O13 Mo4 O6 156.72(12) . . ?
O13 Mo4 O9 95.53(12) . . ?
O13 Mo4 O14 88.40(13) . . ?
O14 Mo4 Mo3 136.31(10) . . ?
O14 Mo4 O2 79.89(12) . . ?
O14 Mo4 O6 83.28(12) . . ?
O25 Mo4 Mo3 100.24(12) . . ?
O25 Mo4 O2 168.67(14) . . ?
O25 Mo4 O6 96.64(14) . . ?
O25 Mo4 O9 101.53(14) . . ?
O25 Mo4 O13 105.82(15) . . ?
O25 Mo4 O14 95.60(15) . . ?
O2 Mo5 Mo6 87.30(7) . . ?
O6 Mo5 Mo6 134.62(8) . . ?
O6 Mo5 O2 72.39(11) . . ?
O10 Mo5 Mo6 48.91(8) . . ?
O10 Mo5 O2 79.84(11) . . ?
O10 Mo5 O6 87.06(12) . . ?
O10 Mo5 O15 161.59(13) . . ?
O11 Mo5 Mo6 47.97(9) . . ?
O11 Mo5 O2 82.84(12) . . ?
O11 Mo5 O6 154.33(12) . . ?
O11 Mo5 O10 95.24(12) . . ?
O11 Mo5 O15 87.57(13) . . ?
O15 Mo5 Mo6 135.36(10) . . ?
O15 Mo5 O2 82.48(12) . . ?
O15 Mo5 O6 82.73(13) . . ?
O20 Mo5 Mo6 100.07(11) . . ?
O20 Mo5 O2 171.23(13) . . ?
O20 Mo5 O6 98.93(14) . . ?
O20 Mo5 O10 101.35(14) . . ?
O20 Mo5 O11 105.62(15) . . ?
O20 Mo5 O15 95.36(14) . . ?
O4 Mo6 Mo5 90.15(7) . . ?
O7 Mo6 Mo5 133.02(8) . . ?
O7 Mo6 O4 75.05(11) . . ?
O10 Mo6 Mo5 48.75(8) . . ?
O10 Mo6 O4 81.79(11) . . ?
O10 Mo6 O7 84.70(11) . . ?
O10 Mo6 O16 159.90(12) . . ?
O11 Mo6 Mo5 48.21(9) . . ?
O11 Mo6 O4 84.68(12) . . ?
O11 Mo6 O7 159.54(12) . . ?
O11 Mo6 O10 95.32(12) . . ?
O11 Mo6 O16 87.89(13) . . ?
O16 Mo6 Mo5 135.75(10) . . ?
O16 Mo6 O4 78.75(11) . . ?
O16 Mo6 O7 85.46(12) . . ?
O21 Mo6 Mo5 99.87(12) . . ?
O21 Mo6 O4 169.30(14) . . ?
O21 Mo6 O7 95.18(14) . . ?
O21 Mo6 O10 101.94(14) . . ?
O21 Mo6 O11 104.78(15) . . ?
O21 Mo6 O16 96.37(15) . . ?
O8 Mn3 O8 84.34(15) . 6_565 ?
O8 Mn3 O9 82.90(11) 6_565 . ?
O8 Mn3 O9 82.90(11) . 6_565 ?
O8 Mn3 O9 96.41(11) 6_565 6_565 ?
O8 Mn3 O9 96.41(11) . . ?
O8 Mn3 O10 179.14(11) . 6_565 ?
O8 Mn3 O10 179.14(11) 6_565 . ?
O8 Mn3 O10 94.82(10) . . ?
O8 Mn3 O10 94.81(11) 6_565 6_565 ?
O9 Mn3 O9 179.07(16) 6_565 . ?
O10 Mn3 O9 83.32(11) 6_565 . ?
O10 Mn3 O9 97.36(11) . . ?
O10 Mn3 O9 83.33(11) . 6_565 ?
O10 Mn3 O9 97.36(11) 6_565 6_565 ?
O10 Mn3 O10 86.03(15) 6_565 . ?
Na2 Mn1 Na1 83.92(8) 10_564 . ?
O3 Mn1 Na1 61.51(9) . . ?
O3 Mn1 Na2 122.29(12) . 10_564 ?
O3 Mn1 O27 159.54(18) . 19_576 ?
O3 Mn1 O32 82.8(2) . 10_564 ?
O3 Mn1 O33 83.87(14) . 19_576 ?
O27 Mn1 Na1 122.91(11) 19_576 . ?
O27 Mn1 Na2 45.51(13) 19_576 10_564 ?
O27 Mn1 O32 78.5(2) 19_576 10_564 ?
O27 Mn1 O33 89.56(14) 19_576 19_576 ?
O28 Mn1 Na1 36.85(10) 10_564 . ?
O28 Mn1 Na2 60.70(12) 10_564 10_564 ?
O28 Mn1 O3 98.36(13) 10_564 . ?
O28 Mn1 O27 88.26(15) 10_564 19_576 ?
O28 Mn1 O31 90.55(15) 10_564 . ?
O28 Mn1 O32 84.7(2) 10_564 10_564 ?
O28 Mn1 O33 177.75(14) 10_564 19_576 ?
O31 Mn1 Na1 103.78(13) . . ?
O31 Mn1 Na2 119.74(14) . 10_564 ?
O31 Mn1 O3 112.90(15) . . ?
O31 Mn1 O27 86.22(19) . 19_576 ?
O31 Mn1 O32 164.1(2) . 10_564 ?
O31 Mn1 O33 88.74(16) . 19_576 ?
O32 Mn1 Na1 81.3(2) 10_564 . ?
O32 Mn1 Na2 45.15(19) 10_564 10_564 ?
O33 Mn1 Na1 145.39(10) 19_576 . ?
O33 Mn1 Na2 117.92(12) 19_576 10_564 ?
O33 Mn1 O32 95.5(3) 19_576 10_564 ?
O26 Mn2 P4 110.58(13) 19_576 . ?
O26 Mn2 O29 136.33(17) 19_576 10_564 ?
O26 Mn2 O30 103.0(2) 19_576 25_565 ?
O26 Mn2 O30 116.01(18) 19_576 . ?
O26 Mn2 O31 91.43(16) 19_576 . ?
O29 Mn2 P4 85.90(11) 10_564 . ?
O29 Mn2 O30 112.19(17) 10_564 25_565 ?
O29 Mn2 O30 98.72(15) 10_564 . ?
O29 Mn2 O31 83.19(15) 10_564 . ?
O30 Mn2 P4 30.39(10) . . ?
O30 Mn2 P4 103.60(18) 25_565 . ?
O30 Mn2 O30 73.26(19) 25_565 . ?
O30 Mn2 O31 133.0(2) 25_565 . ?
O31 Mn2 P4 30.86(11) . . ?
O31 Mn2 O30 60.36(15) . . ?
O1 P1 O2 108.28(16) . . ?
O1 P1 O4 106.43(16) . . ?
O3 P1 O1 110.33(18) . . ?
O3 P1 O2 110.30(18) . . ?
O3 P1 O4 114.10(18) . . ?
O4 P1 O2 107.14(16) . . ?
O16 P2 O17 110.39(17) . . ?
O26 P2 O16 109.1(2) . . ?
O26 P2 O17 108.3(2) . . ?
O27 P2 O16 109.8(2) . . ?
O27 P2 O17 108.7(2) . . ?
O27 P2 O26 110.6(3) . . ?
Na1 P3 Na2 89.01(11) . . ?
O18 P3 Na1 127.58(14) . . ?
O18 P3 Na2 53.37(14) . . ?
O19 P3 Na1 62.80(15) . . ?
O19 P3 Na2 129.16(15) . . ?
O19 P3 O18 110.64(18) . . ?
O28 P3 Na1 44.86(15) . . ?
O28 P3 Na2 56.08(15) . . ?
O28 P3 O18 109.2(2) . . ?
O28 P3 O19 107.5(2) . . ?
O28 P3 O29 114.3(2) . . ?
O29 P3 Na1 125.21(16) . . ?
O29 P3 Na2 122.07(16) . . ?
O29 P3 O18 106.6(2) . . ?
O29 P3 O19 108.6(2) . . ?
O14 P4 Mn2 112.36(13) . . ?
O14 P4 O15 111.89(18) . . ?
O15 P4 Mn2 135.59(14) . . ?
O30 P4 Mn2 55.6(3) . . ?
O30 P4 O14 109.3(2) . . ?
O30 P4 O15 111.6(3) . . ?
O30 P4 O31 105.0(3) . . ?
O31 P4 Mn2 51.5(2) . . ?
O31 P4 O14 111.1(2) . . ?
O31 P4 O15 107.6(2) . . ?
Na2 P5 Na2 98.83(4) 28_656 10_564 ?
Na2 P5 Na2 133.88(12) 28_656 19_576 ?
Na2 P5 Na2 133.87(12) 10_564 . ?
Na2 P5 Na2 98.83(4) 19_576 . ?
Na2 P5 Na2 98.83(4) 28_656 . ?
Na2 P5 Na2 98.83(4) 19_576 10_564 ?
O32 P5 Na2 128.8(3) 10_564 28_656 ?
O32 P5 Na2 115.0(3) . 10_564 ?
O32 P5 Na2 128.8(3) 28_656 . ?
O32 P5 Na2 79.3(4) 10_564 19_576 ?
O32 P5 Na2 79.3(4) 28_656 10_564 ?
O32 P5 Na2 30.3(3) . . ?
O32 P5 Na2 79.3(4) . 28_656 ?
O32 P5 Na2 128.8(3) 19_576 10_564 ?
O32 P5 Na2 30.3(3) 28_656 28_656 ?
O32 P5 Na2 79.3(4) 19_576 . ?
O32 P5 Na2 115.0(3) 28_656 19_576 ?
O32 P5 Na2 128.8(3) . 19_576 ?
O32 P5 Na2 115.0(3) 19_576 28_656 ?
O32 P5 Na2 30.3(3) 19_576 19_576 ?
O32 P5 Na2 30.3(3) 10_564 10_564 ?
O32 P5 Na2 115.0(3) 10_564 . ?
O32 P5 O32 108.5(3) 10_564 19_576 ?
O32 P5 O32 108.5(3) 28_656 10_564 ?
O32 P5 O32 108.5(3) 28_656 . ?
O32 P5 O32 111.4(6) 10_564 . ?
O32 P5 O32 108.5(3) 19_576 . ?
O32 P5 O32 111.4(6) 28_656 19_576 ?
Mn1 Na1 Mn1 99.11(11) . 10_564 ?
P3 Na1 Mn1 58.43(4) . 10_564 ?
P3 Na1 Mn1 58.43(4) 10_564 . ?
P3 Na1 Mn1 120.65(9) . . ?
P3 Na1 Mn1 120.65(9) 10_564 10_564 ?
P3 Na1 P3 178.79(17) 10_564 . ?
O13 Na1 Mn1 140.85(8) . 10_564 ?
O13 Na1 Mn1 83.05(8) 10_564 10_564 ?
O13 Na1 Mn1 140.85(8) 10_564 . ?
O13 Na1 Mn1 83.06(8) . . ?
O13 Na1 P3 93.96(8) . 10_564 ?
O13 Na1 P3 86.66(8) . . ?
O13 Na1 P3 93.96(8) 10_564 . ?
O13 Na1 P3 86.66(8) 10_564 10_564 ?
O13 Na1 O13 119.4(2) 10_564 . ?
O13 Na1 O19 93.88(13) 10_564 . ?
O13 Na1 O19 61.13(11) 10_564 10_564 ?
O13 Na1 O19 61.13(11) . . ?
O13 Na1 O19 93.89(13) . 10_564 ?
O19 Na1 Mn1 87.54(7) 10_564 . ?
O19 Na1 Mn1 125.20(8) . . ?
O19 Na1 Mn1 125.20(8) 10_564 10_564 ?
O19 Na1 Mn1 87.55(7) . 10_564 ?
O19 Na1 P3 29.46(7) . . ?
O19 Na1 P3 151.57(15) 10_564 . ?
O19 Na1 P3 151.57(15) . 10_564 ?
O19 Na1 P3 29.46(7) 10_564 10_564 ?
O19 Na1 O19 131.4(2) 10_564 . ?
O28 Na1 Mn1 32.57(9) 10_564 . ?
O28 Na1 Mn1 107.44(16) . . ?
O28 Na1 Mn1 107.44(16) 10_564 10_564 ?
O28 Na1 Mn1 32.57(9) . 10_564 ?
O28 Na1 P3 151.70(18) . 10_564 ?
O28 Na1 P3 27.21(8) 10_564 10_564 ?
O28 Na1 P3 151.70(18) 10_564 . ?
O28 Na1 P3 27.21(8) . . ?
O28 Na1 O13 109.30(11) 10_564 10_564 ?
O28 Na1 O13 109.30(11) . . ?
O28 Na1 O13 95.27(11) . 10_564 ?
O28 Na1 O13 95.27(11) 10_564 . ?
O28 Na1 O19 56.61(10) 10_564 10_564 ?
O28 Na1 O19 153.45(11) 10_564 . ?
O28 Na1 O19 56.62(10) . . ?
O28 Na1 O19 153.45(11) . 10_564 ?
O28 Na1 O28 130.5(3) 10_564 . ?
Mn1 Na2 Mo2 119.62(9) 10_564 . ?
Mn1 Na2 P3 61.61(6) 10_564 . ?
Mn1 Na2 P5 66.04(6) 10_564 . ?
Co1 Na2 Mo2 119.62(9) 10_564 . ?
Co1 Na2 Mn1 0.0 10_564 10_564 ?
Co1 Na2 P3 61.61(6) 10_564 . ?
Co1 Na2 P5 66.04(6) 10_564 . ?
P3 Na2 Mo2 58.02(5) . . ?
P3 Na2 P5 111.00(10) . . ?
P5 Na2 Mo2 137.34(13) . . ?
O12 Na2 Mo2 29.82(9) . . ?
O12 Na2 Mn1 149.29(15) . 10_564 ?
O12 Na2 Co1 149.29(15) . 10_564 ?
O12 Na2 P3 87.80(12) . . ?
O12 Na2 P5 129.46(16) . . ?
O12 Na2 O18 63.95(12) . . ?
O12 Na2 O28 109.50(16) . . ?
O12 Na2 O33 74.42(14) . . ?
O18 Na2 Mo2 34.91(7) . . ?
O18 Na2 Mn1 86.70(10) . 10_564 ?
O18 Na2 Co1 86.70(10) . 10_564 ?
O18 Na2 P3 27.23(8) . . ?
O18 Na2 P5 135.94(15) . . ?
O18 Na2 O28 53.66(11) . . ?
O27 Na2 Mo2 117.70(18) 28_656 . ?
O27 Na2 Mn1 43.00(11) 28_656 10_564 ?
O27 Na2 Co1 43.00(11) 28_656 10_564 ?
O27 Na2 P3 75.31(15) 28_656 . ?
O27 Na2 P5 94.80(15) 28_656 . ?
O27 Na2 O12 135.7(2) 28_656 . ?
O27 Na2 O18 86.17(18) 28_656 . ?
O27 Na2 O28 70.55(14) 28_656 . ?
O27 Na2 O33 110.7(2) 28_656 . ?
O28 Na2 Mo2 81.09(10) . . ?
O28 Na2 Mn1 40.54(8) . 10_564 ?
O28 Na2 Co1 40.54(8) . 10_564 ?
O28 Na2 P3 26.53(7) . . ?
O28 Na2 P5 85.16(11) . . ?
O32 Na2 Mo2 141.2(3) . . ?
O32 Na2 Mn1 46.1(2) . 10_564 ?
O32 Na2 Co1 46.1(2) . 10_564 ?
O32 Na2 P3 96.9(2) . . ?
O32 Na2 P5 20.0(2) . . ?
O32 Na2 O12 146.2(3) . . ?
O32 Na2 O18 124.0(2) . . ?
O32 Na2 O27 77.3(3) . 28_656 ?
O32 Na2 O28 70.4(2) . . ?
O32 Na2 O33 103.3(2) . . ?
O33 Na2 Mo2 103.53(12) . . ?
O33 Na2 Mn1 136.12(14) . 10_564 ?
O33 Na2 Co1 136.12(14) . 10_564 ?
O33 Na2 P3 159.69(14) . . ?
O33 Na2 P5 88.23(12) . . ?
O33 Na2 O18 132.46(16) . . ?
O33 Na2 O28 173.37(19) . . ?
Mo3 O1 Mo2 100.35(11) . . ?
P1 O1 Mo2 127.84(17) . . ?
P1 O1 Mo3 125.93(17) . . ?
Mo4 O2 Mo5 101.49(11) . . ?
P1 O2 Mo4 124.55(17) . . ?
P1 O2 Mo5 128.20(17) . . ?
P1 O3 Mn1 131.7(2) . . ?
Mo6 O4 Mo1 98.06(11) . . ?
P1 O4 Mo1 127.28(16) . . ?
P1 O4 Mo6 125.66(16) . . ?
Mo2 O5 Mo3 112.35(14) . . ?
Mo5 O6 Mo4 112.70(13) . . ?
Mo1 O7 Mo6 112.01(13) . . ?
Mo1 O8 Mo2 81.97(11) . . ?
Mo1 O8 Mn3 135.59(15) . . ?
Mo2 O8 Mn3 134.09(15) . . ?
Mo3 O9 Mn3 134.57(15) . . ?
Mo4 O9 Mo3 81.88(11) . . ?
Mo4 O9 Mn3 133.23(15) . . ?
Mo5 O10 Mo6 82.34(11) . . ?
Mo5 O10 Mn3 133.24(15) . . ?
Mo6 O10 Mn3 135.76(15) . . ?
Mo6 O11 Mo5 83.81(12) . . ?
Mo1 O12 Na2 153.48(19) . . ?
Mo2 O12 Mo1 83.95(12) . . ?
Mo2 O12 Na2 114.75(16) . . ?
Mo3 O13 Mo4 83.54(12) . . ?
Mo3 O13 Na1 109.87(13) . . ?
Mo4 O13 Na1 156.69(17) . . ?
P4 O14 Mo4 136.4(2) . . ?
P4 O15 Mo5 133.86(19) . . ?
P2 O16 Mo6 138.36(19) . . ?
P2 O17 Mo1 137.53(19) . . ?
Mo2 O18 Na2 94.85(13) . . ?
P3 O18 Mo2 137.35(19) . . ?
P3 O18 Na2 99.40(17) . . ?
Mo3 O19 Na1 99.46(13) . . ?
P3 O19 Mo3 136.1(2) . . ?
P3 O19 Na1 87.74(16) . . ?
Co2 O26 Mn2 0.0 28_656 28_656 ?
P2 O26 Mn2 123.7(3) . 28_656 ?
P2 O26 Co2 123.7(3) . 28_656 ?
Mn1 O27 Na2 91.50(18) 28_656 19_576 ?
Co1 O27 Mn1 0.0 28_656 28_656 ?
Co1 O27 Na2 91.50(18) 28_656 19_576 ?
P2 O27 Mn1 133.3(2) . 28_656 ?
P2 O27 Co1 133.3(2) . 28_656 ?
P2 O27 Na2 135.1(2) . 19_576 ?
Mn1 O28 Na1 110.58(15) 10_564 . ?
Mn1 O28 Na2 78.76(12) 10_564 . ?
Co1 O28 Mn1 0.0 10_564 10_564 ?
Co1 O28 Na1 110.58(15) 10_564 . ?
Co1 O28 Na2 78.76(12) 10_564 . ?
P3 O28 Mn1 135.2(2) . 10_564 ?
P3 O28 Co1 135.2(2) . 10_564 ?
P3 O28 Na1 107.9(2) . . ?
P3 O28 Na2 97.38(18) . . ?
Na1 O28 Na2 124.76(18) . . ?
Co2 O29 Mn2 0.0 10_564 10_564 ?
P3 O29 Mn2 127.0(2) . 10_564 ?
P3 O29 Co2 127.0(2) . 10_564 ?
Mn2 O30 Mn2 106.74(19) 25_565 . ?
Co2 O30 Mn2 106.7 25_565 . ?
Co2 O30 Mn2 0.0 25_565 25_565 ?
P4 O30 Mn2 94.0(3) . . ?
P4 O30 Mn2 159.0(4) . 25_565 ?
P4 O30 Co2 159.0(4) . 25_565 ?
Mn1 O31 Mn2 114.24(17) . . ?
P4 O31 Mn1 143.5(3) . . ?
P4 O31 Mn2 97.7(3) . . ?
Co1 O32 Mn1 0.0 10_564 10_564 ?
P5 O32 Mn1 141.3(4) . 10_564 ?
P5 O32 Co1 141.3(4) . 10_564 ?
P5 O32 Na2 129.7(5) . . ?
Na2 O32 Mn1 88.7(3) . 10_564 ?
Na2 O32 Co1 88.7(3) . 10_564 ?
Mn1 O33 Na2 115.16(19) 28_656 . ?
Co1 O33 Mn1 0.0 28_656 28_656 ?
Co1 O33 Na2 115.16(19) 28_656 . ?

loop_
_platon_missing_refln_index_h
_platon_missing_refln_index_k
_platon_missing_refln_index_l
_platon_missing_refln_theta
0 2 0 1.510
2 2 0 2.136
0 4 0 3.021
1 2 1 1.760
1 1 2 1.456
0 2 2 1.806
1 3 2 2.585
1 2 3 2.249
0 0 4 1.979
0 2 4 2.490
0 0 16 7.941
0 0 20 9.945

_platon_squeeze_details          
;
TITL 111_a.res in I4(1)/acd
CELL   26.9679   26.9679   41.1540     90.00     90.00     90.00
SPGR I41/acd
# Solvent Accessible Volume =      8025
# Electrons Found in S.A.V. =      2697
# Note: Atoms in Void as Cxxx and Qxxx all others
Q101 0.443 0.568 0.063 !       5.69 eA-3
Q102 0.156 0.816 0.366 !       4.33 eA-3
C103 0.992 0.119 0.064 !       4.31 eA-3
C104 0.087 0.495 0.085 !       3.78 eA-3
C105 0.838 0.269 0.162 !       3.18 eA-3
C106 0.022 0.587 0.437 !       3.06 eA-3
C107 0.033 0.251 0.178 !       2.76 eA-3
C108 0.291 0.872 0.198 !       2.63 eA-3
C109 0.586 0.738 0.174 !       2.60 eA-3
C110 0.658 0.596 0.043 !       2.57 eA-3
C111 0.352 0.278 0.358 !       2.56 eA-3
C112 0.053 0.195 0.127 !       2.52 eA-3
C113 0.854 0.894 0.313 !       2.46 eA-3
C114 0.247 0.420 0.135 !       2.36 eA-3
Q115 0.171 0.578 0.154 !       2.24 eA-3
C116 0.905 0.257 0.142 !       2.20 eA-3
C117 0.759 0.016 0.119 !       2.13 eA-3
C118 0.750 0.465 0.369 !       2.06 eA-3
C119 0.892 0.955 0.417 !       1.97 eA-3
Q120 0.814 0.908 0.031 !       1.69 eA-3
C121 0.220 0.454 0.149 !       1.60 eA-3
Q122 0.227 0.776 0.078 !       1.58 eA-3
C123 0.324 0.134 0.351 !       1.58 eA-3
C124 0.741 0.945 0.389 !       1.57 eA-3
Q125 0.742 0.182 0.254 !       1.55 eA-3
Q126 0.275 0.857 0.420 !       1.49 eA-3
C127 0.218 0.463 0.129 !       1.48 eA-3
Q128 0.930 0.089 0.055 !       1.42 eA-3
Q129 0.876 0.240 0.033 !       1.40 eA-3
Q130 0.307 0.730 0.282 !       1.32 eA-3
Q131 0.212 0.362 0.219 !       1.21 eA-3
Q132 0.273 0.194 0.219 !       1.17 eA-3
Q133 0.296 0.797 0.257 !       1.17 eA-3
Q134 0.818 0.317 0.469 !       1.14 eA-3
C135 0.563 0.884 0.615 !       1.13 eA-3
C136 0.063 0.384 0.115 !       1.13 eA-3
Q137 0.523 0.282 0.157 !       1.11 eA-3
C138 0.930 0.738 0.374 !       1.09 eA-3
C139 0.614 0.320 0.358 !       1.05 eA-3
Q140 0.091 0.128 0.220 !       1.04 eA-3
Q141 0.312 0.196 0.220 !       0.94 eA-3
Q142 0.812 0.696 0.720 !       0.94 eA-3
Q143 0.054 0.438 0.970 !       0.94 eA-3
Q144 0.405 0.812 0.181 !       0.93 eA-3
Q145 0.769 0.187 0.493 !       0.91 eA-3
Q146 0.731 0.313 0.007 !       0.91 eA-3
Q147 0.231 0.187 0.993 !       0.91 eA-3
Q148 0.555 0.029 0.013 !       0.90 eA-3
Q149 0.562 0.712 0.180 !       0.88 eA-3
Q150 0.523 0.014 0.033 !       0.88 eA-3
C151 0.720 0.497 0.335 !       0.88 eA-3
C152 0.181 0.485 0.161 !       0.85 eA-3
Q153 0.874 0.182 0.258 !       0.85 eA-3
Q154 0.022 0.800 0.124 !       0.85 eA-3
Q155 0.931 0.924 0.032 !       0.84 eA-3
Q156 0.233 0.204 0.984 !       0.84 eA-3
Q157 0.564 0.010 0.000 !       0.84 eA-3
Q158 0.814 0.125 0.413 !       0.83 eA-3
Q159 0.866 0.449 0.228 !       0.82 eA-3
Q160 0.968 0.249 0.376 !       0.82 eA-3
Q161 0.219 0.413 0.277 !       0.82 eA-3
Q162 0.967 0.126 0.412 !       0.81 eA-3
Q163 0.303 0.773 0.338 !       0.81 eA-3
Q164 0.766 0.305 0.015 !       0.81 eA-3
C165 0.013 0.808 0.399 !       0.80 eA-3
Q166 0.795 0.358 0.392 !       0.79 eA-3
Q167 0.775 0.282 0.990 !       0.79 eA-3
Q168 0.454 0.405 0.483 !       0.79 eA-3
Q169 0.696 0.016 0.033 !       0.79 eA-3
Q170 0.291 0.759 0.438 !       0.78 eA-3
Q171 0.239 0.743 0.828 !       0.78 eA-3
Q172 0.739 0.243 0.328 !       0.78 eA-3
Q173 0.036 0.500 0.250 !       0.78 eA-3
Q174 0.275 0.720 0.995 !       0.78 eA-3
Q175 0.121 0.835 0.273 !       0.78 eA-3
C176 0.618 0.663 0.128 !       0.78 eA-3
Q177 0.133 0.280 0.468 !       0.78 eA-3
Q178 0.229 0.455 0.306 !       0.77 eA-3
Q179 0.452 0.041 0.468 !       0.77 eA-3
Q180 0.529 0.265 0.165 !       0.77 eA-3
Q181 0.299 0.054 0.472 !       0.77 eA-3
Q182 0.201 0.446 0.028 !       0.77 eA-3
Q183 0.482 0.627 0.290 !       0.76 eA-3
Q184 0.102 0.278 0.455 !       0.76 eA-3
Q185 0.299 0.445 0.965 !       0.76 eA-3
Q186 0.429 0.722 0.187 !       0.76 eA-3
Q187 0.225 0.836 0.488 !       0.76 eA-3
Q188 0.484 0.905 0.038 !       0.75 eA-3
Q189 0.416 0.839 0.367 !       0.75 eA-3
Q190 0.852 0.416 0.381 !       0.75 eA-3
Q191 0.648 0.084 0.119 !       0.75 eA-3
Q192 0.148 0.416 0.881 !       0.75 eA-3
Q193 0.853 0.214 0.439 !       0.75 eA-3
Q194 0.366 0.256 0.182 !       0.74 eA-3
C195 0.252 0.112 0.358 !       0.74 eA-3
C196 0.125 0.355 0.155 !       0.74 eA-3
Q197 0.817 0.705 0.229 !       0.74 eA-3
Q198 0.490 0.881 0.431 !       0.74 eA-3
Q199 0.388 0.073 0.178 !       0.74 eA-3
;
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.500 -0.250 0.125 1009 338 ' '
2 1.000 0.250 0.125 1009 338 ' '
3 0.500 0.250 0.375 1008 338 ' '
4 1.000 -0.250 0.375 1008 338 ' '
5 0.000 0.250 0.625 1009 338 ' '
6 0.500 -0.250 0.625 1009 338 ' '
7 0.000 -0.250 0.875 1008 338 ' '
8 0.500 0.250 0.875 1008 338 ' '

_platon_squeeze_void_probe_radius 1.20

_olex2_submission_special_instructions 'No special instructions were received'
